# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2016

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mo_mayr146_0m
_database_code_depnum_ccdc_archive 'CCDC 1437129'
_audit_update_record             
;
2015-11-15 deposited with the CCDC.
2015-12-18 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Cs3Na[Nb2W4O19] 10H2O'
_chemical_formula_sum            'H20 Cs3 Na Nb2 O29 W4'
_chemical_formula_weight         1827.10

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           146
_space_group_name_H-M_alt        'R 3 :H'
_space_group_name_Hall           'R 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'

_cell_length_a                   11.6472(15)
_cell_length_b                   11.6472(15)
_cell_length_c                   19.117(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     2245.9(6)
_cell_formula_units_Z            3
_cell_measurement_temperature    173(2)
_cell_measurement_reflns_used    3117
_cell_measurement_theta_min      2.28
_cell_measurement_theta_max      27.5

_exptl_crystal_description       cut-block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.053
_exptl_crystal_F_000             2418
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.040
_exptl_absorpt_coefficient_mu    19.752
_shelx_estimated_absorpt_T_min   0.269
_shelx_estimated_absorpt_T_max   0.505
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.5553
_exptl_absorpt_correction_T_max  0.7460
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      173(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'sealed tube'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            12477
_diffrn_reflns_av_unetI/netI     0.0566
_diffrn_reflns_av_R_equivalents  0.0586
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_theta_min         2.283
_diffrn_reflns_theta_max         30.117
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.948
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.948
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.948
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             2686
_reflns_number_gt                2220
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         1.000
_reflns_Friedel_fraction_max     0.948
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick 2013)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'



_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0218P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.000042(17)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.35(2)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         2686
_refine_ls_number_parameters     120
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0497
_refine_ls_R_factor_gt           0.0325
_refine_ls_wR_factor_ref         0.0581
_refine_ls_wR_factor_gt          0.0537
_refine_ls_goodness_of_fit_ref   1.006
_refine_ls_restrained_S_all      1.006
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.52317(7) 0.23845(7) 1.00049(3) 0.01766(18) Uani 0.767 1 d . . P . .
Nb1 Nb -0.52317(7) 0.23845(7) 1.00049(3) 0.01766(18) Uani 0.233 1 d . . P . .
W2 W -0.42883(8) 0.14229(8) 0.85800(3) 0.0173(2) Uani 0.566 1 d . . P . .
Nb2 Nb -0.42883(8) 0.14229(8) 0.85800(3) 0.0173(2) Uani 0.434 1 d . . P . .
Cs1 Cs -0.86325(10) 0.27364(10) 0.97183(6) 0.0330(2) Uani 1 1 d . . . . .
Na1 Na -0.6667 0.6667 0.9269(5) 0.022(2) Uani 1 3 d S T P . .
O1 O -0.3333 0.3333 0.9307(11) 0.012(2) Uani 1 3 d S T P . .
O2 O -0.3324(10) 0.1032(9) 0.9317(6) 0.021(3) Uani 1 1 d . . . . .
O3 O -0.5638(10) 0.1035(9) 0.9315(6) 0.020(3) Uani 1 1 d . . . . .
O4 O -0.4113(9) 0.1783(10) 1.0451(6) 0.020(3) Uani 1 1 d . . . . .
O5 O -0.2548(10) 0.2570(10) 0.8147(7) 0.022(3) Uani 1 1 d . . . . .
O6 O -0.6681(12) 0.1664(12) 1.0510(6) 0.035(3) Uani 1 1 d . . . . .
O7 O -0.5002(11) -0.0001(11) 0.8061(6) 0.024(3) Uani 1 1 d . . . . .
O1S O -0.8082(11) 0.0964(11) 0.8618(7) 0.034(4) Uani 1 1 d . . . . .
O2S O -0.7614(11) 0.7610(11) 0.8506(7) 0.043(3) Uani 1 1 d . . . . .
O3S O -0.5698(11) 0.8599(10) 1.0025(6) 0.027(3) Uani 1 1 d . . . . .
O4S O -1.0000 0.0000 1.0577(11) 0.067(7) Uani 1 3 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O6 1.752(12) . ?
W1 O2 1.919(10) 3_455 ?
W1 O3 1.921(10) . ?
W1 O4 1.957(10) . ?
W1 O4 1.965(10) 3_455 ?
W1 O1 2.334(12) . ?
W1 Cs1 4.2156(13) 3_345 ?
W1 Cs1 4.2169(13) . ?
W2 O7 1.746(11) . ?
W2 O5 1.946(11) 3_455 ?
W2 O5 1.967(11) . ?
W2 O3 1.985(11) . ?
W2 O2 1.992(10) . ?
W2 O1 2.376(12) . ?
Cs1 O2S 3.098(13) 2_575 ?
Cs1 O4S 3.212(11) . ?
Cs1 O1S 3.228(12) . ?
Cs1 O1S 3.236(12) 2_465 ?
Cs1 O7 3.259(11) 4_455 ?
Cs1 O2 3.285(9) 3_455 ?
Cs1 O3 3.289(10) 2_465 ?
Cs1 O6 3.443(12) . ?
Cs1 O6 3.449(13) 2_465 ?
Cs1 O3S 3.481(11) 3_355 ?
Cs1 O3S 3.485(11) 2_575 ?
Cs1 Na1 4.057(2) . ?
Na1 O2S 2.400(12) 2_575 ?
Na1 O2S 2.400(12) . ?
Na1 O2S 2.400(12) 3_355 ?
Na1 O3S 2.427(13) . ?
Na1 O3S 2.427(13) 2_575 ?
Na1 O3S 2.427(13) 3_355 ?
Na1 Cs1 4.057(2) 2_575 ?
Na1 Cs1 4.057(2) 3_355 ?
O1 Nb1 2.334(12) 2_565 ?
O1 W1 2.334(12) 2_565 ?
O1 Nb1 2.334(12) 3_455 ?
O1 W1 2.334(12) 3_455 ?
O1 Nb2 2.376(12) 2_565 ?
O1 W2 2.376(12) 2_565 ?
O1 Nb2 2.376(12) 3_455 ?
O1 W2 2.376(12) 3_455 ?
O2 Nb1 1.919(10) 2_565 ?
O2 W1 1.919(10) 2_565 ?
O2 Cs1 3.285(9) 2_565 ?
O3 Cs1 3.289(10) 3_345 ?
O4 Nb1 1.965(10) 2_565 ?
O4 W1 1.965(10) 2_565 ?
O5 Nb2 1.946(11) 2_565 ?
O5 W2 1.946(11) 2_565 ?
O6 Cs1 3.449(13) 3_345 ?
O7 Cs1 3.259(11) 7_544 ?
O1S Cs1 3.236(12) 3_345 ?
O2S Cs1 3.099(13) 3_355 ?
O3S Cs1 3.481(11) 2_575 ?
O3S Cs1 3.485(11) 3_355 ?
O4S Cs1 3.212(11) 3_345 ?
O4S Cs1 3.212(11) 2_465 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 W1 O2 101.2(5) . 3_455 ?
O6 W1 O3 101.6(5) . . ?
O2 W1 O3 88.1(6) 3_455 . ?
O6 W1 O4 104.1(5) . . ?
O2 W1 O4 154.7(4) 3_455 . ?
O3 W1 O4 86.6(5) . . ?
O6 W1 O4 104.0(5) . 3_455 ?
O2 W1 O4 86.7(5) 3_455 3_455 ?
O3 W1 O4 154.3(4) . 3_455 ?
O4 W1 O4 87.4(6) . 3_455 ?
O6 W1 O1 178.5(6) . . ?
O2 W1 O1 77.7(4) 3_455 . ?
O3 W1 O1 77.4(4) . . ?
O4 W1 O1 77.0(5) . . ?
O4 W1 O1 76.9(5) 3_455 . ?
O6 W1 Cs1 52.7(4) . 3_345 ?
O2 W1 Cs1 97.4(3) 3_455 3_345 ?
O3 W1 Cs1 48.9(3) . 3_345 ?
O4 W1 Cs1 97.7(3) . 3_345 ?
O4 W1 Cs1 156.7(3) 3_455 3_345 ?
O1 W1 Cs1 126.4(3) . 3_345 ?
O6 W1 Cs1 52.5(4) . . ?
O2 W1 Cs1 48.7(3) 3_455 . ?
O3 W1 Cs1 97.5(3) . . ?
O4 W1 Cs1 156.6(3) . . ?
O4 W1 Cs1 97.8(3) 3_455 . ?
O1 W1 Cs1 126.4(3) . . ?
Cs1 W1 Cs1 69.07(3) 3_345 . ?
O7 W2 O5 103.7(5) . 3_455 ?
O7 W2 O5 104.2(5) . . ?
O5 W2 O5 87.5(6) 3_455 . ?
O7 W2 O3 103.9(5) . . ?
O5 W2 O3 87.0(4) 3_455 . ?
O5 W2 O3 151.9(4) . . ?
O7 W2 O2 103.9(5) . . ?
O5 W2 O2 152.4(4) 3_455 . ?
O5 W2 O2 86.9(5) . . ?
O3 W2 O2 85.4(5) . . ?
O7 W2 O1 178.9(6) . . ?
O5 W2 O1 77.0(5) 3_455 . ?
O5 W2 O1 76.7(5) . . ?
O3 W2 O1 75.3(4) . . ?
O2 W2 O1 75.3(4) . . ?
O2S Cs1 O4S 162.4(4) 2_575 . ?
O2S Cs1 O1S 83.1(3) 2_575 . ?
O4S Cs1 O1S 81.8(4) . . ?
O2S Cs1 O1S 83.3(3) 2_575 2_465 ?
O4S Cs1 O1S 81.7(4) . 2_465 ?
O1S Cs1 O1S 62.4(4) . 2_465 ?
O2S Cs1 O7 127.8(3) 2_575 4_455 ?
O4S Cs1 O7 69.9(4) . 4_455 ?
O1S Cs1 O7 138.0(3) . 4_455 ?
O1S Cs1 O7 137.8(3) 2_465 4_455 ?
O2S Cs1 O2 72.8(3) 2_575 3_455 ?
O4S Cs1 O2 105.91(19) . 3_455 ?
O1S Cs1 O2 56.8(3) . 3_455 ?
O1S Cs1 O2 116.4(3) 2_465 3_455 ?
O7 Cs1 O2 101.3(3) 4_455 3_455 ?
O2S Cs1 O3 72.9(3) 2_575 2_465 ?
O4S Cs1 O3 106.0(2) . 2_465 ?
O1S Cs1 O3 116.3(3) . 2_465 ?
O1S Cs1 O3 56.9(3) 2_465 2_465 ?
O7 Cs1 O3 101.3(3) 4_455 2_465 ?
O2 Cs1 O3 145.6(3) 3_455 2_465 ?
O2S Cs1 O6 122.4(3) 2_575 . ?
O4S Cs1 O6 60.3(2) . . ?
O1S Cs1 O6 71.1(3) . . ?
O1S Cs1 O6 123.2(3) 2_465 . ?
O7 Cs1 O6 68.1(3) 4_455 . ?
O2 Cs1 O6 49.8(3) 3_455 . ?
O3 Cs1 O6 164.5(3) 2_465 . ?
O2S Cs1 O6 122.6(3) 2_575 2_465 ?
O4S Cs1 O6 60.3(2) . 2_465 ?
O1S Cs1 O6 123.1(3) . 2_465 ?
O1S Cs1 O6 70.9(3) 2_465 2_465 ?
O7 Cs1 O6 68.1(3) 4_455 2_465 ?
O2 Cs1 O6 164.4(3) 3_455 2_465 ?
O3 Cs1 O6 50.0(3) 2_465 2_465 ?
O6 Cs1 O6 114.6(4) . 2_465 ?
O2S Cs1 O3S 63.6(3) 2_575 3_355 ?
O4S Cs1 O3S 130.6(3) . 3_355 ?
O1S Cs1 O3S 109.5(2) . 3_355 ?
O1S Cs1 O3S 146.9(4) 2_465 3_355 ?
O7 Cs1 O3S 71.1(3) 4_455 3_355 ?
O2 Cs1 O3S 54.6(2) 3_455 3_355 ?
O3 Cs1 O3S 110.3(3) 2_465 3_355 ?
O6 Cs1 O3S 77.7(3) . 3_355 ?
O6 Cs1 O3S 127.2(3) 2_465 3_355 ?
O2S Cs1 O3S 63.7(3) 2_575 2_575 ?
O4S Cs1 O3S 130.7(3) . 2_575 ?
O1S Cs1 O3S 146.7(4) . 2_575 ?
O1S Cs1 O3S 109.6(2) 2_465 2_575 ?
O7 Cs1 O3S 71.1(3) 4_455 2_575 ?
O2 Cs1 O3S 110.3(3) 3_455 2_575 ?
O3 Cs1 O3S 54.6(2) 2_465 2_575 ?
O6 Cs1 O3S 127.1(3) . 2_575 ?
O6 Cs1 O3S 77.9(3) 2_465 2_575 ?
O3S Cs1 O3S 58.0(3) 3_355 2_575 ?
O2S Cs1 Na1 36.2(2) 2_575 . ?
O4S Cs1 Na1 161.5(3) . . ?
O1S Cs1 Na1 113.8(2) . . ?
O1S Cs1 Na1 113.9(2) 2_465 . ?
O7 Cs1 Na1 91.6(2) 4_455 . ?
O2 Cs1 Na1 76.94(18) 3_455 . ?
O3 Cs1 Na1 76.91(19) 2_465 . ?
O6 Cs1 Na1 113.6(2) . . ?
O6 Cs1 Na1 113.7(2) 2_465 . ?
O3S Cs1 Na1 36.6(2) 3_355 . ?
O3S Cs1 Na1 36.6(2) 2_575 . ?
O2S Na1 O2S 87.0(5) 2_575 . ?
O2S Na1 O2S 87.0(5) 2_575 3_355 ?
O2S Na1 O2S 87.0(5) . 3_355 ?
O2S Na1 O3S 179.2(6) 2_575 . ?
O2S Na1 O3S 92.5(4) . . ?
O2S Na1 O3S 92.4(4) 3_355 . ?
O2S Na1 O3S 92.5(4) 2_575 2_575 ?
O2S Na1 O3S 92.4(4) . 2_575 ?
O2S Na1 O3S 179.2(6) 3_355 2_575 ?
O3S Na1 O3S 88.1(5) . 2_575 ?
O2S Na1 O3S 92.4(4) 2_575 3_355 ?
O2S Na1 O3S 179.2(6) . 3_355 ?
O2S Na1 O3S 92.5(4) 3_355 3_355 ?
O3S Na1 O3S 88.1(5) . 3_355 ?
O3S Na1 O3S 88.1(5) 2_575 3_355 ?
O2S Na1 Cs1 121.1(3) 2_575 2_575 ?
O2S Na1 Cs1 121.2(3) . 2_575 ?
O2S Na1 Cs1 49.6(3) 3_355 2_575 ?
O3S Na1 Cs1 58.7(3) . 2_575 ?
O3S Na1 Cs1 131.2(4) 2_575 2_575 ?
O3S Na1 Cs1 58.8(3) 3_355 2_575 ?
O2S Na1 Cs1 49.6(3) 2_575 . ?
O2S Na1 Cs1 121.1(3) . . ?
O2S Na1 Cs1 121.2(3) 3_355 . ?
O3S Na1 Cs1 131.2(4) . . ?
O3S Na1 Cs1 58.8(3) 2_575 . ?
O3S Na1 Cs1 58.7(3) 3_355 . ?
Cs1 Na1 Cs1 115.64(9) 2_575 . ?
O2S Na1 Cs1 121.2(3) 2_575 3_355 ?
O2S Na1 Cs1 49.6(3) . 3_355 ?
O2S Na1 Cs1 121.1(3) 3_355 3_355 ?
O3S Na1 Cs1 58.8(3) . 3_355 ?
O3S Na1 Cs1 58.7(3) 2_575 3_355 ?
O3S Na1 Cs1 131.2(4) 3_355 3_355 ?
Cs1 Na1 Cs1 115.63(9) 2_575 3_355 ?
Cs1 Na1 Cs1 115.64(9) . 3_355 ?
Nb1 O1 W1 0.00(3) 2_565 2_565 ?
Nb1 O1 Nb1 90.6(6) 2_565 3_455 ?
W1 O1 Nb1 90.6(6) 2_565 3_455 ?
Nb1 O1 W1 90.6(6) 2_565 3_455 ?
W1 O1 W1 90.6(6) 2_565 3_455 ?
Nb1 O1 W1 0.00(4) 3_455 3_455 ?
Nb1 O1 W1 90.6(6) 2_565 . ?
W1 O1 W1 90.6(6) 2_565 . ?
Nb1 O1 W1 90.6(6) 3_455 . ?
W1 O1 W1 90.6(6) 3_455 . ?
Nb1 O1 W2 90.09(3) 2_565 . ?
W1 O1 W2 90.09(3) 2_565 . ?
Nb1 O1 W2 179.1(8) 3_455 . ?
W1 O1 W2 179.1(8) 3_455 . ?
W1 O1 W2 90.11(3) . . ?
Nb1 O1 Nb2 90.11(3) 2_565 2_565 ?
W1 O1 Nb2 90.11(3) 2_565 2_565 ?
Nb1 O1 Nb2 90.09(3) 3_455 2_565 ?
W1 O1 Nb2 90.09(3) 3_455 2_565 ?
W1 O1 Nb2 179.1(8) . 2_565 ?
W2 O1 Nb2 89.2(6) . 2_565 ?
Nb1 O1 W2 90.11(3) 2_565 2_565 ?
W1 O1 W2 90.11(3) 2_565 2_565 ?
Nb1 O1 W2 90.09(3) 3_455 2_565 ?
W1 O1 W2 90.09(3) 3_455 2_565 ?
W1 O1 W2 179.1(8) . 2_565 ?
W2 O1 W2 89.2(6) . 2_565 ?
Nb2 O1 W2 0.00(2) 2_565 2_565 ?
Nb1 O1 Nb2 179.1(8) 2_565 3_455 ?
W1 O1 Nb2 179.1(8) 2_565 3_455 ?
Nb1 O1 Nb2 90.11(3) 3_455 3_455 ?
W1 O1 Nb2 90.11(3) 3_455 3_455 ?
W1 O1 Nb2 90.09(3) . 3_455 ?
W2 O1 Nb2 89.2(6) . 3_455 ?
Nb2 O1 Nb2 89.2(6) 2_565 3_455 ?
W2 O1 Nb2 89.2(6) 2_565 3_455 ?
Nb1 O1 W2 179.1(8) 2_565 3_455 ?
W1 O1 W2 179.1(8) 2_565 3_455 ?
Nb1 O1 W2 90.11(3) 3_455 3_455 ?
W1 O1 W2 90.11(3) 3_455 3_455 ?
W1 O1 W2 90.09(3) . 3_455 ?
W2 O1 W2 89.2(6) . 3_455 ?
Nb2 O1 W2 89.2(6) 2_565 3_455 ?
W2 O1 W2 89.2(6) 2_565 3_455 ?
Nb2 O1 W2 0.00(4) 3_455 3_455 ?
Nb1 O2 W1 0.00(2) 2_565 2_565 ?
Nb1 O2 W2 116.9(5) 2_565 . ?
W1 O2 W2 116.9(5) 2_565 . ?
Nb1 O2 Cs1 105.2(4) 2_565 2_565 ?
W1 O2 Cs1 105.2(4) 2_565 2_565 ?
W2 O2 Cs1 137.8(4) . 2_565 ?
W1 O3 W2 117.2(5) . . ?
W1 O3 Cs1 105.0(4) . 3_345 ?
W2 O3 Cs1 137.9(4) . 3_345 ?
W1 O4 Nb1 115.5(5) . 2_565 ?
W1 O4 W1 115.5(5) . 2_565 ?
Nb1 O4 W1 0.00(5) 2_565 2_565 ?
Nb2 O5 W2 0.00(5) 2_565 2_565 ?
Nb2 O5 W2 117.0(6) 2_565 . ?
W2 O5 W2 117.0(6) 2_565 . ?
W1 O6 Cs1 103.7(5) . . ?
W1 O6 Cs1 103.4(5) . 3_345 ?
Cs1 O6 Cs1 87.8(3) . 3_345 ?
W2 O7 Cs1 135.3(5) . 7_544 ?
Cs1 O1S Cs1 95.4(3) . 3_345 ?
Na1 O2S Cs1 94.2(4) . 3_355 ?
Na1 O3S Cs1 84.7(3) . 2_575 ?
Na1 O3S Cs1 84.6(3) . 3_355 ?
Cs1 O3S Cs1 160.6(4) 2_575 3_355 ?
Cs1 O4S Cs1 96.2(4) 3_345 2_465 ?
Cs1 O4S Cs1 96.2(4) 3_345 . ?
Cs1 O4S Cs1 96.2(4) 2_465 . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 W1 O6 Cs1 -0.2(5) 3_455 . . . ?
O3 W1 O6 Cs1 -90.6(4) . . . . ?
O4 W1 O6 Cs1 180.0(4) . . . . ?
O4 W1 O6 Cs1 89.1(5) 3_455 . . . ?
Cs1 W1 O6 Cs1 -91.1(5) 3_345 . . . ?
O2 W1 O6 Cs1 90.8(4) 3_455 . . 3_345 ?
O3 W1 O6 Cs1 0.5(5) . . . 3_345 ?
O4 W1 O6 Cs1 -89.0(5) . . . 3_345 ?
O4 W1 O6 Cs1 -179.8(4) 3_455 . . 3_345 ?
Cs1 W1 O6 Cs1 91.1(5) . . . 3_345 ?
O5 W2 O7 Cs1 45.6(8) 3_455 . . 7_544 ?
O5 W2 O7 Cs1 -45.3(8) . . . 7_544 ?
O3 W2 O7 Cs1 135.8(7) . . . 7_544 ?
O2 W2 O7 Cs1 -135.6(7) . . . 7_544 ?

_refine_diff_density_max         1.192
_refine_diff_density_min         -1.075
_refine_diff_density_rms         0.265

_shelxl_version_number           2013-4

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mo_may110_0m
_database_code_depnum_ccdc_archive 'CCDC 1437130'
_audit_update_record             
;
2015-11-15 deposited with the CCDC.
2015-12-18 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'Cs4[Nb2W4O19] 4H2O'
_chemical_formula_sum            'H8 Cs4 Nb1.97 O23 W4.03'
_chemical_formula_weight         1832.11

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   9.6119(8)
_cell_length_b                   11.8087(10)
_cell_length_c                   11.2532(9)
_cell_angle_alpha                90
_cell_angle_beta                 90.929(4)
_cell_angle_gamma                90
_cell_volume                     1277.12(18)
_cell_formula_units_Z            2
_cell_measurement_temperature    173(2)
_cell_measurement_reflns_used    6775
_cell_measurement_theta_min      2.50
_cell_measurement_theta_max      37.03

_exptl_crystal_description       cut-block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.764
_exptl_crystal_F_000             1582
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.090
_exptl_crystal_size_mid          0.070
_exptl_crystal_size_min          0.060
_exptl_absorpt_coefficient_mu    24.655
_shelx_estimated_absorpt_T_min   0.215
_shelx_estimated_absorpt_T_max   0.319
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.5981
_exptl_absorpt_correction_T_max  0.7485
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      173(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'sealed tube'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            42881
_diffrn_reflns_av_unetI/netI     0.0744
_diffrn_reflns_av_R_equivalents  0.0848
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         2.500
_diffrn_reflns_theta_max         43.405
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             9627
_reflns_number_gt                6273
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2013 (Sheldrick 2013)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'


_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0071P)²+21.0175P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00156(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         9627
_refine_ls_number_parameters     155
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0897
_refine_ls_R_factor_gt           0.0468
_refine_ls_wR_factor_ref         0.1037
_refine_ls_wR_factor_gt          0.0869
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_restrained_S_all      1.016
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.73580(3) 0.00422(2) 0.55538(2) 0.01589(7) Uani 0.871(4) 1 d . . P A 1
W2 W 0.52763(4) 0.17885(2) 0.40451(2) 0.01682(9) Uani 0.623(4) 1 d . . P A 1
W3 W 0.44591(4) 0.09392(3) 0.67739(3) 0.01537(9) Uani 0.523(4) 1 d . . P A 1
Nb1 Nb 0.73580(3) 0.00422(2) 0.55538(2) 0.01589(7) Uani 0.129(4) 1 d . . P A 2
Nb2 Nb 0.52763(4) 0.17885(2) 0.40451(2) 0.01682(9) Uani 0.377(4) 1 d . . P A 2
Nb3 Nb 0.44591(4) 0.09392(3) 0.67739(3) 0.01537(9) Uani 0.477(4) 1 d . . P A 2
Cs1 Cs 0.96819(6) -0.26263(4) 0.45362(4) 0.02922(12) Uani 1 1 d . . . . .
Cs2 Cs 0.89411(5) 0.05853(4) 0.19650(4) 0.02572(11) Uani 1 1 d . . . . .
O1 O 0.5000 0.0000 0.5000 0.0124(9) Uani 1 2 d S . P . .
O2 O 0.7136(5) 0.1437(5) 0.4703(4) 0.0228(9) Uani 1 1 d . . . . .
O3 O 0.6462(5) 0.0757(4) 0.6876(4) 0.0205(8) Uani 1 1 d . . . . .
O4 O 0.4811(6) 0.2173(4) 0.5645(4) 0.0207(9) Uani 1 1 d . . . . .
O5 O 0.6734(6) -0.1386(5) 0.6202(4) 0.0268(11) Uani 1 1 d . . . . .
O6 O 0.5663(6) 0.0697(5) 0.2809(4) 0.0245(10) Uani 1 1 d . . . . .
O7 O 0.7342(5) -0.0727(4) 0.4034(4) 0.0202(8) Uani 1 1 d . . . . .
O8 O 0.9089(6) 0.0069(8) 0.5984(5) 0.0447(18) Uani 1 1 d . . . . .
O9 O 0.547(2) 0.3070(5) 0.3307(7) 0.132(7) Uani 1 1 d . . . . .
O10 O 0.4029(8) 0.1654(15) 0.8089(9) 0.135(7) Uani 1 1 d . . . . .
O1S O 1.2609(7) -0.3461(6) 0.3562(5) 0.0362(13) Uani 1 1 d . . . . .
O2S O 0.7612(9) 0.0656(7) -0.0531(6) 0.0460(17) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O8 1.726(6) . ?
W1 O2 1.916(5) . ?
W1 O3 1.926(5) . ?
W1 O7 1.936(4) . ?
W1 O5 1.937(6) . ?
W1 O1 2.3414(3) . ?
W1 Cs1 4.0391(6) . ?
W1 Cs1 4.1745(7) 3_756 ?
W1 Cs2 4.3859(6) . ?
W2 O9 1.737(6) . ?
W2 O4 1.917(4) . ?
W2 O6 1.936(5) . ?
W2 O2 1.968(5) . ?
W2 O5 2.005(6) 3_656 ?
W2 O1 2.3864(3) . ?
W2 Cs1 4.0898(6) 2_655 ?
W2 Cs2 4.4915(7) . ?
W3 O10 1.758(6) . ?
W3 O3 1.939(5) . ?
W3 O7 1.958(5) 3_656 ?
W3 O4 1.966(5) . ?
W3 O6 1.993(6) 3_656 ?
W3 O1 2.3493(3) . ?
W3 Cs2 4.0107(6) 3_656 ?
W3 Cs2 4.1402(6) 4_566 ?
Cs1 O10 3.049(6) 2_646 ?
Cs1 O1S 3.192(7) . ?
Cs1 O2S 3.211(8) 2_645 ?
Cs1 O7 3.220(5) . ?
Cs1 O8 3.299(9) 3_756 ?
Cs1 O9 3.304(9) 2_645 ?
Cs1 O6 3.312(5) 2_645 ?
Cs1 O2 3.461(5) 3_756 ?
Cs1 O8 3.625(8) . ?
Cs1 O5 3.723(5) . ?
Cs2 O9 3.041(7) 2_645 ?
Cs2 O8 3.060(6) 3_756 ?
Cs2 O2S 3.068(7) . ?
Cs2 O4 3.155(4) 4_665 ?
Cs2 O7 3.210(5) . ?
Cs2 O6 3.309(5) . ?
Cs2 O10 3.50(2) 4_665 ?
Cs2 O1S 3.561(7) 2_755 ?
Cs2 O2 3.699(5) . ?
Cs2 Nb3 4.0107(6) 3_656 ?
Cs2 W3 4.0107(6) 3_656 ?
Cs2 Nb3 4.1402(6) 4_665 ?
O1 Nb1 2.3414(3) 3_656 ?
O1 W1 2.3414(3) 3_656 ?
O1 Nb3 2.3493(3) 3_656 ?
O1 W3 2.3493(3) 3_656 ?
O1 W2 2.3864(3) 3_656 ?
O1 Nb2 2.3864(3) 3_656 ?
O2 Cs1 3.460(5) 3_756 ?
O4 Cs2 3.155(4) 4_566 ?
O5 Nb2 2.005(6) 3_656 ?
O5 W2 2.005(6) 3_656 ?
O6 Nb3 1.993(6) 3_656 ?
O6 W3 1.993(6) 3_656 ?
O6 Cs1 3.312(5) 2_655 ?
O7 Nb3 1.958(5) 3_656 ?
O7 W3 1.958(5) 3_656 ?
O8 Cs2 3.060(6) 3_756 ?
O8 Cs1 3.299(9) 3_756 ?
O9 Cs2 3.041(7) 2_655 ?
O9 Cs1 3.304(9) 2_655 ?
O10 Cs1 3.049(6) 2_656 ?
O10 Cs2 3.50(2) 4_566 ?
O1S Cs2 3.561(7) 2_745 ?
O2S Cs1 3.211(8) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O8 W1 O2 102.9(3) . . ?
O8 W1 O3 102.5(3) . . ?
O2 W1 O3 87.8(2) . . ?
O8 W1 O7 104.5(3) . . ?
O2 W1 O7 87.9(2) . . ?
O3 W1 O7 153.0(2) . . ?
O8 W1 O5 102.3(3) . . ?
O2 W1 O5 154.8(2) . . ?
O3 W1 O5 86.9(2) . . ?
O7 W1 O5 85.7(2) . . ?
O8 W1 O1 179.1(2) . . ?
O2 W1 O1 77.63(14) . . ?
O3 W1 O1 76.83(14) . . ?
O7 W1 O1 76.17(14) . . ?
O5 W1 O1 77.14(16) . . ?
O8 W1 Cs1 63.8(3) . . ?
O2 W1 Cs1 125.92(16) . . ?
O3 W1 Cs1 144.80(14) . . ?
O7 W1 Cs1 51.69(14) . . ?
O5 W1 Cs1 66.64(16) . . ?
O1 W1 Cs1 116.442(12) . . ?
O8 W1 Cs1 48.6(3) . 3_756 ?
O2 W1 Cs1 55.23(14) . 3_756 ?
O3 W1 Cs1 90.67(15) . 3_756 ?
O7 W1 Cs1 108.50(15) . 3_756 ?
O5 W1 Cs1 149.44(16) . 3_756 ?
O1 W1 Cs1 131.784(12) . 3_756 ?
Cs1 W1 Cs1 100.552(12) . 3_756 ?
O8 W1 Cs2 84.7(2) . . ?
O2 W1 Cs2 56.73(15) . . ?
O3 W1 Cs2 144.43(15) . . ?
O7 W1 Cs2 41.70(15) . . ?
O5 W1 Cs2 126.04(15) . . ?
O1 W1 Cs2 96.131(10) . . ?
Cs1 W1 Cs2 69.590(10) . . ?
Cs1 W1 Cs2 67.913(10) 3_756 . ?
O9 W2 O4 105.7(3) . . ?
O9 W2 O6 102.3(3) . . ?
O4 W2 O6 152.0(2) . . ?
O9 W2 O2 105.1(7) . . ?
O4 W2 O2 85.5(2) . . ?
O6 W2 O2 86.9(2) . . ?
O9 W2 O5 104.4(7) . 3_656 ?
O4 W2 O5 87.0(2) . 3_656 ?
O6 W2 O5 86.5(2) . 3_656 ?
O2 W2 O5 150.5(2) . 3_656 ?
O9 W2 O1 178.2(3) . . ?
O4 W2 O1 75.96(13) . . ?
O6 W2 O1 76.02(16) . . ?
O2 W2 O1 75.60(15) . . ?
O5 W2 O1 74.86(14) 3_656 . ?
O9 W2 Cs1 51.6(3) . 2_655 ?
O4 W2 Cs1 153.08(13) . 2_655 ?
O6 W2 Cs1 53.11(15) . 2_655 ?
O2 W2 Cs1 112.50(14) . 2_655 ?
O5 W2 Cs1 85.88(13) 3_656 2_655 ?
O1 W2 Cs1 126.599(12) . 2_655 ?
O9 W2 Cs2 86.3(5) . . ?
O4 W2 Cs2 139.60(16) . . ?
O6 W2 Cs2 41.75(17) . . ?
O2 W2 Cs2 54.12(14) . . ?
O5 W2 Cs2 127.95(15) 3_656 . ?
O1 W2 Cs2 92.788(11) . . ?
Cs1 W2 Cs2 61.287(11) 2_655 . ?
O10 W3 O3 104.5(3) . . ?
O10 W3 O7 103.5(3) . 3_656 ?
O3 W3 O7 151.99(18) . 3_656 ?
O10 W3 O4 103.5(7) . . ?
O3 W3 O4 86.5(2) . . ?
O7 W3 O4 87.4(2) 3_656 . ?
O10 W3 O6 104.6(7) . 3_656 ?
O3 W3 O6 86.6(2) . 3_656 ?
O7 W3 O6 86.0(2) 3_656 3_656 ?
O4 W3 O6 151.91(18) . 3_656 ?
O10 W3 O1 179.0(4) . . ?
O3 W3 O1 76.41(13) . . ?
O7 W3 O1 75.59(13) 3_656 . ?
O4 W3 O1 75.99(12) . . ?
O6 W3 O1 75.92(13) 3_656 . ?
O10 W3 Cs2 73.4(5) . 3_656 ?
O3 W3 Cs2 138.01(14) . 3_656 ?
O7 W3 Cs2 52.25(14) 3_656 3_656 ?
O4 W3 Cs2 135.30(16) . 3_656 ?
O6 W3 Cs2 55.26(15) 3_656 3_656 ?
O1 W3 Cs2 106.355(13) . 3_656 ?
O10 W3 Cs2 56.7(6) . 4_566 ?
O3 W3 Cs2 103.11(15) . 4_566 ?
O7 W3 Cs2 92.56(15) 3_656 4_566 ?
O4 W3 Cs2 47.24(13) . 4_566 ?
O6 W3 Cs2 160.33(14) 3_656 4_566 ?
O1 W3 Cs2 122.724(13) . 4_566 ?
Cs2 W3 Cs2 109.098(10) 3_656 4_566 ?
O10 Cs1 O1S 82.4(3) 2_646 . ?
O10 Cs1 O2S 77.9(2) 2_646 2_645 ?
O1S Cs1 O2S 122.60(18) . 2_645 ?
O10 Cs1 O7 128.4(3) 2_646 . ?
O1S Cs1 O7 140.52(15) . . ?
O2S Cs1 O7 91.12(17) 2_645 . ?
O10 Cs1 O8 105.6(3) 2_646 3_756 ?
O1S Cs1 O8 84.35(16) . 3_756 ?
O2S Cs1 O8 152.90(17) 2_645 3_756 ?
O7 Cs1 O8 65.31(14) . 3_756 ?
O10 Cs1 O9 158.3(4) 2_646 2_645 ?
O1S Cs1 O9 76.6(3) . 2_645 ?
O2S Cs1 O9 118.4(3) 2_645 2_645 ?
O7 Cs1 O9 68.7(3) . 2_645 ?
O8 Cs1 O9 67.1(2) 3_756 2_645 ?
O10 Cs1 O6 124.5(4) 2_646 2_645 ?
O1S Cs1 O6 67.60(14) . 2_645 ?
O2S Cs1 O6 80.78(15) 2_645 2_645 ?
O7 Cs1 O6 102.47(13) . 2_645 ?
O8 Cs1 O6 115.93(14) 3_756 2_645 ?
O9 Cs1 O6 51.30(14) 2_645 2_645 ?
O10 Cs1 O2 63.3(2) 2_646 3_756 ?
O1S Cs1 O2 55.24(14) . 3_756 ?
O2S Cs1 O2 141.19(15) 2_645 3_756 ?
O7 Cs1 O2 111.90(13) . 3_756 ?
O8 Cs1 O2 49.83(14) 3_756 3_756 ?
O9 Cs1 O2 99.4(3) 2_645 3_756 ?
O6 Cs1 O2 121.09(13) 2_645 3_756 ?
O10 Cs1 O8 85.1(4) 2_646 . ?
O1S Cs1 O8 124.84(15) . . ?
O2S Cs1 O8 106.51(17) 2_645 . ?
O7 Cs1 O8 49.68(13) . . ?
O8 Cs1 O8 48.34(19) 3_756 . ?
O9 Cs1 O8 102.26(16) 2_645 . ?
O6 Cs1 O8 150.32(14) 2_645 . ?
O2 Cs1 O8 71.17(13) 3_756 . ?
O10 Cs1 O5 88.3(3) 2_646 . ?
O1S Cs1 O5 167.60(13) . . ?
O2S Cs1 O5 62.64(16) 2_645 . ?
O7 Cs1 O5 43.87(10) . . ?
O8 Cs1 O5 90.39(14) 3_756 . ?
O9 Cs1 O5 111.6(3) 2_645 . ?
O6 Cs1 O5 124.71(13) 2_645 . ?
O2 Cs1 O5 113.12(13) 3_756 . ?
O8 Cs1 O5 45.72(14) . . ?
O10 Cs1 W1 100.8(4) 2_646 . ?
O1S Cs1 W1 146.39(12) . . ?
O2S Cs1 W1 90.46(14) 2_645 . ?
O7 Cs1 W1 28.16(8) . . ?
O8 Cs1 W1 62.44(11) 3_756 . ?
O9 Cs1 W1 93.72(19) 2_645 . ?
O6 Cs1 W1 130.07(10) 2_645 . ?
O2 Cs1 W1 95.96(10) 3_756 . ?
O8 Cs1 W1 25.29(9) . . ?
O5 Cs1 W1 28.53(9) . . ?
O9 Cs2 O8 73.4(3) 2_645 3_756 ?
O9 Cs2 O2S 90.6(3) 2_645 . ?
O8 Cs2 O2S 160.2(2) 3_756 . ?
O9 Cs2 O4 136.1(2) 2_645 4_665 ?
O8 Cs2 O4 113.67(18) 3_756 4_665 ?
O2S Cs2 O4 69.86(17) . 4_665 ?
O9 Cs2 O7 72.2(2) 2_645 . ?
O8 Cs2 O7 68.21(16) 3_756 . ?
O2S Cs2 O7 118.69(17) . . ?
O4 Cs2 O7 151.69(12) 4_665 . ?
O9 Cs2 O6 104.4(3) 2_645 . ?
O8 Cs2 O6 111.96(14) 3_756 . ?
O2S Cs2 O6 82.96(17) . . ?
O4 Cs2 O6 111.25(14) 4_665 . ?
O7 Cs2 O6 48.81(12) . . ?
O9 Cs2 O10 160.7(3) 2_645 4_665 ?
O8 Cs2 O10 87.23(19) 3_756 4_665 ?
O2S Cs2 O10 108.24(18) . 4_665 ?
O4 Cs2 O10 51.91(14) 4_665 4_665 ?
O7 Cs2 O10 101.36(14) . 4_665 ?
O6 Cs2 O10 82.90(17) . 4_665 ?
O9 Cs2 O1S 96.7(3) 2_645 2_755 ?
O8 Cs2 O1S 68.84(16) 3_756 2_755 ?
O2S Cs2 O1S 102.36(17) . 2_755 ?
O4 Cs2 O1S 53.25(14) 4_665 2_755 ?
O7 Cs2 O1S 137.03(12) . 2_755 ?
O6 Cs2 O1S 158.27(15) . 2_755 ?
O10 Cs2 O1S 75.42(17) 4_665 2_755 ?
O9 Cs2 O2 116.13(18) 2_645 . ?
O8 Cs2 O2 74.54(14) 3_756 . ?
O2S Cs2 O2 124.13(17) . . ?
O4 Cs2 O2 107.18(12) 4_665 . ?
O7 Cs2 O2 44.82(12) . . ?
O6 Cs2 O2 44.63(11) . . ?
O10 Cs2 O2 56.93(14) 4_665 . ?
O1S Cs2 O2 120.21(13) 2_755 . ?
O9 Cs2 Nb3 75.6(3) 2_645 3_656 ?
O8 Cs2 Nb3 96.76(14) 3_756 3_656 ?
O2S Cs2 Nb3 90.37(14) . 3_656 ?
O4 Cs2 Nb3 140.07(10) 4_665 3_656 ?
O7 Cs2 Nb3 28.84(8) . 3_656 ?
O6 Cs2 Nb3 29.66(10) . 3_656 ?
O10 Cs2 Nb3 107.79(13) 4_665 3_656 ?
O1S Cs2 Nb3 165.30(9) 2_755 3_656 ?
O2 Cs2 Nb3 55.36(8) . 3_656 ?
O9 Cs2 W3 75.6(3) 2_645 3_656 ?
O8 Cs2 W3 96.76(14) 3_756 3_656 ?
O2S Cs2 W3 90.37(14) . 3_656 ?
O4 Cs2 W3 140.07(10) 4_665 3_656 ?
O7 Cs2 W3 28.84(8) . 3_656 ?
O6 Cs2 W3 29.66(10) . 3_656 ?
O10 Cs2 W3 107.79(13) 4_665 3_656 ?
O1S Cs2 W3 165.30(9) 2_755 3_656 ?
O2 Cs2 W3 55.36(8) . 3_656 ?
O9 Cs2 Nb3 160.1(3) 2_645 4_665 ?
O8 Cs2 Nb3 102.46(16) 3_756 4_665 ?
O2S Cs2 Nb3 88.52(15) . 4_665 ?
O4 Cs2 Nb3 27.23(8) 4_665 4_665 ?
O7 Cs2 Nb3 125.15(9) . 4_665 ?
O6 Cs2 Nb3 95.23(10) . 4_665 ?
O10 Cs2 Nb3 24.84(10) 4_665 4_665 ?
O1S Cs2 Nb3 64.19(11) 2_755 4_665 ?
O2 Cs2 Nb3 80.33(8) . 4_665 ?
Nb3 Cs2 Nb3 124.242(14) 3_656 4_665 ?
W1 O1 W1 180.0 . 3_656 ?
W1 O1 W3 89.448(11) . . ?
W1 O1 W3 90.551(11) 3_656 . ?
Nb1 O1 Nb3 89.449(11) 3_656 3_656 ?
W1 O1 W3 90.552(11) . 3_656 ?
W1 O1 W3 89.449(11) 3_656 3_656 ?
W3 O1 W3 180.0 . 3_656 ?
W1 O1 W2 89.238(11) . . ?
W1 O1 W2 90.762(11) 3_656 . ?
W3 O1 W2 89.575(12) . . ?
W3 O1 W2 90.425(12) 3_656 . ?
W1 O1 W2 90.761(11) . 3_656 ?
W1 O1 W2 89.239(11) 3_656 3_656 ?
W3 O1 W2 90.426(12) . 3_656 ?
W3 O1 W2 89.574(12) 3_656 3_656 ?
W2 O1 W2 180.0 . 3_656 ?
Nb1 O1 Nb2 89.239(11) 3_656 3_656 ?
Nb3 O1 Nb2 89.574(12) 3_656 3_656 ?
W1 O2 W2 117.5(2) . . ?
W1 O2 Cs1 97.72(18) . 3_756 ?
W2 O2 Cs1 143.3(2) . 3_756 ?
W1 O2 Cs2 97.6(2) . . ?
W2 O2 Cs2 100.35(16) . . ?
Cs1 O2 Cs2 83.80(11) 3_756 . ?
W1 O3 W3 117.3(2) . . ?
W2 O4 W3 118.5(2) . . ?
W2 O4 Cs2 135.14(19) . 4_566 ?
W3 O4 Cs2 105.53(17) . 4_566 ?
W1 O5 W2 117.2(2) . 3_656 ?
W1 O5 Cs1 84.84(18) . . ?
Nb2 O5 Cs1 125.2(2) 3_656 . ?
W2 O5 Cs1 125.2(2) 3_656 . ?
W2 O6 W3 117.6(2) . 3_656 ?
W2 O6 Cs2 115.3(2) . . ?
Nb3 O6 Cs2 95.09(18) 3_656 . ?
W3 O6 Cs2 95.09(18) 3_656 . ?
W2 O6 Cs1 99.0(2) . 2_655 ?
Nb3 O6 Cs1 139.6(2) 3_656 2_655 ?
W3 O6 Cs1 139.6(2) 3_656 2_655 ?
Cs2 O6 Cs1 83.02(12) . 2_655 ?
W1 O7 W3 117.7(2) . 3_656 ?
W1 O7 Cs2 114.6(2) . . ?
Nb3 O7 Cs2 98.91(16) 3_656 . ?
W3 O7 Cs2 98.91(16) 3_656 . ?
W1 O7 Cs1 100.16(16) . . ?
Nb3 O7 Cs1 127.0(2) 3_656 . ?
W3 O7 Cs1 127.0(2) 3_656 . ?
Cs2 O7 Cs1 97.02(12) . . ?
W1 O8 Cs2 142.1(4) . 3_756 ?
W1 O8 Cs1 108.2(4) . 3_756 ?
Cs2 O8 Cs1 98.40(18) 3_756 3_756 ?
W1 O8 Cs1 90.9(3) . . ?
Cs2 O8 Cs1 91.0(2) 3_756 . ?
Cs1 O8 Cs1 131.66(19) 3_756 . ?
W2 O9 Cs2 157.0(5) . 2_655 ?
W2 O9 Cs1 104.1(3) . 2_655 ?
Cs2 O9 Cs1 98.68(17) 2_655 2_655 ?
W3 O10 Cs1 140.7(4) . 2_656 ?
W3 O10 Cs2 98.5(7) . 4_566 ?
Cs1 O10 Cs2 93.7(4) 2_656 4_566 ?
Cs1 O1S Cs2 169.5(2) . 2_745 ?
Cs2 O2S Cs1 88.63(19) . 2_655 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 W1 O8 Cs2 143.3(6) . . . 3_756 ?
O3 W1 O8 Cs2 52.7(7) . . . 3_756 ?
O7 W1 O8 Cs2 -125.6(6) . . . 3_756 ?
O5 W1 O8 Cs2 -36.8(6) . . . 3_756 ?
Cs1 W1 O8 Cs2 -92.8(6) . . . 3_756 ?
Cs1 W1 O8 Cs2 132.3(7) 3_756 . . 3_756 ?
Cs2 W1 O8 Cs2 -162.6(6) . . . 3_756 ?
O2 W1 O8 Cs1 10.9(3) . . . 3_756 ?
O3 W1 O8 Cs1 -79.7(2) . . . 3_756 ?
O7 W1 O8 Cs1 102.1(2) . . . 3_756 ?
O5 W1 O8 Cs1 -169.2(2) . . . 3_756 ?
Cs1 W1 O8 Cs1 134.8(3) . . . 3_756 ?
Cs2 W1 O8 Cs1 65.03(17) . . . 3_756 ?
O2 W1 O8 Cs1 -123.91(19) . . . . ?
O3 W1 O8 Cs1 145.47(17) . . . . ?
O7 W1 O8 Cs1 -32.8(2) . . . . ?
O5 W1 O8 Cs1 56.0(2) . . . . ?
Cs1 W1 O8 Cs1 -134.8(3) 3_756 . . . ?
Cs2 W1 O8 Cs1 -69.81(11) . . . . ?
O4 W2 O9 Cs2 26(2) . . . 2_655 ?
O6 W2 O9 Cs2 -154(2) . . . 2_655 ?
O2 W2 O9 Cs2 -64(2) . . . 2_655 ?
O5 W2 O9 Cs2 117(2) 3_656 . . 2_655 ?
Cs1 W2 O9 Cs2 -171(3) 2_655 . . 2_655 ?
Cs2 W2 O9 Cs2 -115(2) . . . 2_655 ?
O4 W2 O9 Cs1 -163.5(4) . . . 2_655 ?
O6 W2 O9 Cs1 16.9(7) . . . 2_655 ?
O2 W2 O9 Cs1 107.0(5) . . . 2_655 ?
O5 W2 O9 Cs1 -72.6(5) 3_656 . . 2_655 ?
Cs2 W2 O9 Cs1 55.7(5) . . . 2_655 ?
O3 W3 O10 Cs1 -10.2(15) . . . 2_656 ?
O7 W3 O10 Cs1 169.4(12) 3_656 . . 2_656 ?
O4 W3 O10 Cs1 -100.1(14) . . . 2_656 ?
O6 W3 O10 Cs1 80.0(14) 3_656 . . 2_656 ?
Cs2 W3 O10 Cs1 126.2(15) 3_656 . . 2_656 ?
Cs2 W3 O10 Cs1 -106.5(15) 4_566 . . 2_656 ?
O3 W3 O10 Cs2 96.4(2) . . . 4_566 ?
O7 W3 O10 Cs2 -84.1(3) 3_656 . . 4_566 ?
O4 W3 O10 Cs2 6.5(3) . . . 4_566 ?
O6 W3 O10 Cs2 -173.43(19) 3_656 . . 4_566 ?
Cs2 W3 O10 Cs2 -127.3(2) 3_656 . . 4_566 ?

_refine_diff_density_max         5.933
_refine_diff_density_min         -4.251
_refine_diff_density_rms         0.504

_shelxl_version_number           2013-4

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_may40_a
_database_code_depnum_ccdc_archive 'CCDC 1437131'
_audit_update_record             
;
2015-11-15 deposited with the CCDC.
2015-12-18 downloaded from the CCDC.
;



_audit_creation_method           SHELXTL

_chemical_name_systematic        
;

 ?

;

_chemical_name_common            ?

_chemical_melting_point          ?

_chemical_formula_moiety         Cs4Na2[Nb4W2O19]12H2O

_chemical_formula_sum            'H24 Cs4 Na2 Nb3.89 O31 W2.11'

_chemical_formula_weight         1846.70



loop_

_atom_type_symbol

_atom_type_description

_atom_type_scat_dispersion_real

_atom_type_scat_dispersion_imag

_atom_type_scat_source












O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'



_symmetry_cell_setting           Monoclinic

_symmetry_space_group_name_H-M   P2(1)/n



loop_

_symmetry_equiv_pos_as_xyz




'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'



_cell_length_a                   9.5760(3)

_cell_length_b                   13.5844(4)

_cell_length_c                   12.3503(4)

_cell_angle_alpha                90.00

_cell_angle_beta                 90.0790(12)

_cell_angle_gamma                90.00

_cell_volume                     1606.58(9)

_cell_formula_units_Z            2

_cell_measurement_temperature    150(2)

_cell_measurement_reflns_used    9966

_cell_measurement_theta_min      2.23

_cell_measurement_theta_max      52.17



_exptl_crystal_description       block

_exptl_crystal_colour            colorless

_exptl_crystal_size_max          0.16

_exptl_crystal_size_mid          0.14

_exptl_crystal_size_min          0.08

_exptl_crystal_density_meas      ?

_exptl_crystal_density_diffrn    3.817

_exptl_crystal_density_method    'not measured'

_exptl_crystal_F_000             1659

_exptl_absorpt_coefficient_mu    13.446

_exptl_absorpt_correction_type   multi-scan

_exptl_absorpt_correction_T_min  0.2222

_exptl_absorpt_correction_T_max  0.4126

_exptl_absorpt_process_details   SADABS



_exptl_special_details           
;

 ?

;



_diffrn_ambient_temperature      150(2)

_diffrn_radiation_wavelength     0.71073

_diffrn_radiation_type           MoK\a

_diffrn_radiation_source         'fine-focus sealed tube'

_diffrn_radiation_monochromator  graphite

_diffrn_measurement_device_type  'Bruker APEX-II CCD'

_diffrn_measurement_method       'φ and ω scans'

_diffrn_detector_area_resol_mean ?

_diffrn_standards_number         0

_diffrn_standards_interval_count ?

_diffrn_standards_interval_time  ?

_diffrn_standards_decay_%        ?

_diffrn_reflns_number            45150

_diffrn_reflns_av_R_equivalents  0.0299

_diffrn_reflns_av_sigmaI/netI    0.0231

_diffrn_reflns_limit_h_min       -17

_diffrn_reflns_limit_h_max       17

_diffrn_reflns_limit_k_min       -24

_diffrn_reflns_limit_k_max       18

_diffrn_reflns_limit_l_min       -22

_diffrn_reflns_limit_l_max       22

_diffrn_reflns_theta_min         2.23

_diffrn_reflns_theta_max         40.00

_reflns_number_total             9955

_reflns_number_gt                9814

_reflns_threshold_expression     >2sigma(I)



_computing_data_collection       'Bruker APEX2'

_computing_cell_refinement       'Bruker SAINT'

_computing_data_reduction        'Bruker SAINT'

_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'

_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'

_computing_molecular_graphics    'Bruker SHELXTL'

_computing_publication_material  'Bruker SHELXTL'



_refine_special_details          
;

 Refinement of F² against ALL reflections.  The weighted R-factor wR and

 goodness of fit S are based on F², conventional R-factors R are based

 on F, with F set to zero for negative F². The threshold expression of

 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is

 not relevant to the choice of reflections for refinement.  R-factors based

 on F² are statistically about twice as large as those based on F, and R-

 factors based on ALL data will be even larger.

;



_refine_ls_structure_factor_coef Fsqd

_refine_ls_matrix_type           full

_refine_ls_weighting_scheme      calc

_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0400P)²+10.9107P] where P=(Fo²+2Fc²)/3'

_atom_sites_solution_primary     direct

_atom_sites_solution_secondary   difmap

_atom_sites_solution_hydrogens   difmap

_refine_ls_hydrogen_treatment    refall

_refine_ls_extinction_method     SHELXL

_refine_ls_extinction_coef       0.00439(15)

_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^

_refine_ls_number_reflns         9955

_refine_ls_number_parameters     248

_refine_ls_number_restraints     12

_refine_ls_R_factor_all          0.0318

_refine_ls_R_factor_gt           0.0310

_refine_ls_wR_factor_ref         0.0921

_refine_ls_wR_factor_gt          0.0917

_refine_ls_goodness_of_fit_ref   1.261

_refine_ls_restrained_S_all      1.260

_refine_ls_shift/su_max          0.004

_refine_ls_shift/su_mean         0.000



loop_

_atom_site_label

_atom_site_type_symbol

_atom_site_fract_x

_atom_site_fract_y

_atom_site_fract_z

_atom_site_U_iso_or_equiv

_atom_site_adp_type

_atom_site_occupancy

_atom_site_symmetry_multiplicity

_atom_site_calc_flag

_atom_site_refinement_flags

_atom_site_disorder_assembly

_atom_site_disorder_group





































W1 W 1.179789(16) 0.386899(12) 1.034998(12) 0.00418(5) Uani 0.498(2) 1 d P . .
W2 W 0.838075(19) 0.369236(14) 0.991789(14) 0.00410(5) Uani 0.319(2) 1 d P . .
W3 W 0.95665(2) 0.514759(15) 1.185200(15) 0.00421(6) Uani 0.235(2) 1 d P . .
Nb1 Nb 1.179789(16) 0.386899(12) 1.034998(12) 0.00418(5) Uani 0.502(2) 1 d P .
.
Nb2 Nb 0.838075(19) 0.369236(14) 0.991789(14) 0.00410(5) Uani 0.681(2) 1 d P .
.
Nb3 Nb 0.95665(2) 0.514759(15) 1.185200(15) 0.00421(6) Uani 0.765(2) 1 d P . .
Cs1 Cs 0.45571(2) 0.253662(16) 0.828164(18) 0.01132(5) Uani 1 1 d . . .
Cs2 Cs 0.05846(2) 0.217376(15) 0.714347(17) 0.01001(5) Uani 1 1 d . . .
Na1 Na -0.03432(18) -0.02164(13) 0.86172(14) 0.0117(3) Uani 1 1 d . . .
O1 O 1.0000 0.5000 1.0000 0.0043(4) Uani 1 2 d S . .
O2 O 1.0159(2) 0.30081(17) 1.0211(2) 0.0074(3) Uani 1 1 d . . .
O3 O 1.1122(2) 0.41913(18) 1.18099(19) 0.0070(3) Uani 1 1 d . . .
O4 O 0.8324(3) 0.40536(19) 1.14585(19) 0.0078(3) Uani 1 1 d . . .
O5 O 1.3128(3) 0.3018(2) 1.0614(2) 0.0098(4) Uani 1 1 d . . .
O6 O 0.9021(3) 0.38202(18) 0.84140(19) 0.0071(3) Uani 1 1 d . . .
O7 O 0.7202(2) 0.48665(18) 0.96522(19) 0.0071(3) Uani 1 1 d . . .
O8 O 0.7200(3) 0.26870(19) 0.9846(2) 0.0092(4) Uani 1 1 d . . .
O9 O 0.9303(3) 0.5325(2) 1.3270(2) 0.0110(4) Uani 1 1 d . . .
O10 O 0.8180(2) 0.60550(18) 1.12273(19) 0.0071(3) Uani 1 1 d . . .
O11 O 0.3307(3) 0.3789(2) 0.6315(3) 0.0146(5) Uani 1 1 d D . .
O12 O 0.4807(3) 0.4917(2) 0.8345(2) 0.0122(4) Uani 1 1 d D . .
O13 O 0.3757(4) 0.0877(3) 0.9946(3) 0.0179(5) Uani 1 1 d D . .
O14 O 0.6905(3) 0.3545(2) 0.6965(2) 0.0138(4) Uani 1 1 d D . .
O15 O 0.0937(3) 0.1062(2) 0.9577(3) 0.0142(4) Uani 1 1 d D . .
O16 O -0.1913(3) 0.1096(3) 0.8385(3) 0.0173(5) Uani 1 1 d D . .
H11A H 0.287(11) 0.416(7) 0.692(6) 0.06(3) Uiso 1 1 d D . .
H11B H 0.310(6) 0.336(4) 0.569(3) 0.001(11) Uiso 1 1 d D . .
H12A H 0.384(5) 0.502(8) 0.861(9) 0.06(3) Uiso 1 1 d D . .
H12B H 0.543(8) 0.481(6) 0.897(5) 0.03(2) Uiso 1 1 d D . .
H13A H 0.405(8) 0.055(5) 1.063(4) 0.022(19) Uiso 1 1 d D . .
H13B H 0.381(8) 0.035(4) 0.939(5) 0.020(18) Uiso 1 1 d D . .
H14A H 0.738(9) 0.308(6) 0.645(6) 0.04(3) Uiso 1 1 d D . .
H14B H 0.770(5) 0.371(6) 0.744(5) 0.017(17) Uiso 1 1 d D . .
H15A H 0.038(9) 0.166(5) 0.978(8) 0.04(3) Uiso 1 1 d D . .
H15B H 0.198(2) 0.101(10) 0.956(11) 0.07(4) Uiso 1 1 d D . .
H16A H -0.281(5) 0.091(7) 0.803(7) 0.03(2) Uiso 1 1 d D . .
H16B H -0.212(7) 0.168(3) 0.883(5) 0.008(14) Uiso 1 1 d D . .






_geom_special_details            
;

 All esds (except the esd in the dihedral angle between two l.s. planes)

 are estimated using the full covariance matrix.  The cell esds are taken

 into account individually in the estimation of esds in distances, angles

 and torsion angles; correlations between esds in cell parameters are only

 used when they are defined by crystal symmetry.  An approximate (isotropic)

 treatment of cell esds is used for estimating esds involving l.s. planes.

;



loop_

_geom_bond_atom_site_label_1

_geom_bond_atom_site_label_2

_geom_bond_distance

_geom_bond_site_symmetry_2

_geom_bond_publ_flag





















































































W1 O5 1.750(2) . ?
W1 O10 1.951(2) 3_767 ?
W1 O2 1.965(2) . ?
W1 O3 1.966(2) . ?
W1 O7 1.967(2) 3_767 ?
W1 O1 2.34722(16) . ?
W1 Nb3 3.2982(3) 3_767 ?
W1 Cs1 4.0989(3) 1_655 ?
W1 Cs2 4.4766(3) 4_766 ?
W2 O8 1.775(2) . ?
W2 O6 1.964(2) . ?
W2 O4 1.966(2) . ?
W2 O2 1.973(2) . ?
W2 O7 1.981(2) . ?
W2 O1 2.36000(19) . ?
W2 Cs2 4.0161(3) 4_666 ?
W2 Cs1 4.4649(3) . ?
W3 O9 1.786(3) . ?
W3 O4 1.964(2) . ?
W3 O10 1.968(2) . ?
W3 O6 1.976(2) 3_767 ?
W3 O3 1.977(2) . ?
W3 O1 2.3338(2) . ?
W3 Nb1 3.2982(3) 3_767 ?
W3 Cs2 3.8473(3) 3_667 ?
W3 Cs1 4.0514(3) 4_666 ?
Cs1 O14 3.096(3) . ?
Cs1 O13 3.146(4) . ?
Cs1 O8 3.188(3) . ?
Cs1 O11 3.197(3) . ?
Cs1 O12 3.244(3) . ?
Cs1 O5 3.257(3) 1_455 ?
Cs1 O10 3.302(2) 3_667 ?
Cs1 O3 3.327(2) 4_565 ?
Cs1 O4 3.335(3) 4_565 ?
Cs1 Na1 3.9228(17) 2_556 ?
Cs1 Nb3 4.0514(3) 4_565 ?
Cs1 W3 4.0514(3) 4_565 ?
Cs2 O5 3.026(3) 4_465 ?
Cs2 O6 3.117(2) 1_455 ?
Cs2 O12 3.146(3) 2_546 ?
Cs2 O16 3.197(4) . ?
Cs2 O4 3.223(2) 4_565 ?
Cs2 O8 3.239(3) 4_565 ?
Cs2 O10 3.351(2) 3_667 ?
Cs2 O15 3.380(3) . ?
Cs2 O9 3.437(3) 3_667 ?
Cs2 O11 3.559(3) . ?
Cs2 Na1 3.8273(18) . ?
Cs2 W3 3.8473(3) 3_667 ?
Na1 O16 2.349(4) . ?
Na1 O14 2.363(3) 2_546 ?
Na1 O11 2.374(4) 2_546 ?
Na1 O15 2.433(3) . ?
Na1 O12 2.484(3) 2_546 ?
Na1 O15 2.573(4) 3_557 ?
Na1 Na1 3.527(3) 3_557 ?
Na1 Cs1 3.9228(17) 2_546 ?
O1 Nb3 2.3338(2) 3_767 ?
O1 W3 2.3338(2) 3_767 ?
O1 Nb1 2.34722(16) 3_767 ?
O1 W1 2.34722(16) 3_767 ?
O1 W2 2.36000(19) 3_767 ?
O1 Nb2 2.36000(19) 3_767 ?
O3 Cs1 3.327(2) 4_666 ?
O4 Cs2 3.223(2) 4_666 ?
O4 Cs1 3.335(2) 4_666 ?
O5 Cs2 3.026(3) 4_766 ?
O5 Cs1 3.257(3) 1_655 ?
O6 Nb3 1.976(2) 3_767 ?
O6 W3 1.976(2) 3_767 ?
O6 Cs2 3.117(2) 1_655 ?
O7 Nb1 1.967(2) 3_767 ?
O7 W1 1.967(2) 3_767 ?
O8 Cs2 3.239(3) 4_666 ?
O9 Cs2 3.437(3) 3_667 ?
O10 Nb1 1.951(2) 3_767 ?
O10 W1 1.951(2) 3_767 ?
O10 Cs1 3.302(2) 3_667 ?
O10 Cs2 3.351(2) 3_667 ?
O11 Na1 2.374(4) 2_556 ?
O12 Na1 2.484(3) 2_556 ?
O12 Cs2 3.146(3) 2_556 ?
O14 Na1 2.363(3) 2_556 ?
O15 Na1 2.573(4) 3_557 ?



loop_

_geom_angle_atom_site_label_1

_geom_angle_atom_site_label_2

_geom_angle_atom_site_label_3

_geom_angle

_geom_angle_site_symmetry_1

_geom_angle_site_symmetry_3

_geom_angle_publ_flag































































































































































































































































































































































O5 W1 O10 102.24(11) . 3_767 ?
O5 W1 O2 101.80(11) . . ?
O10 W1 O2 87.36(10) 3_767 . ?
O5 W1 O3 102.52(11) . . ?
O10 W1 O3 155.24(10) 3_767 . ?
O2 W1 O3 87.07(10) . . ?
O5 W1 O7 102.86(11) . 3_767 ?
O10 W1 O7 86.93(10) 3_767 3_767 ?
O2 W1 O7 155.34(10) . 3_767 ?
O3 W1 O7 88.15(10) . 3_767 ?
O5 W1 O1 179.53(9) . . ?
O10 W1 O1 77.90(7) 3_767 . ?
O2 W1 O1 77.75(7) . . ?
O3 W1 O1 77.34(7) . . ?
O7 W1 O1 77.60(7) 3_767 . ?
O5 W1 Nb3 135.10(9) . 3_767 ?
O10 W1 Nb3 32.86(7) 3_767 3_767 ?
O2 W1 Nb3 81.58(7) . 3_767 ?
O3 W1 Nb3 122.38(7) . 3_767 ?
O7 W1 Nb3 80.65(7) 3_767 3_767 ?
O1 W1 Nb3 45.040(4) . 3_767 ?
O5 W1 Cs1 49.82(9) . 1_655 ?
O10 W1 Cs1 52.65(7) 3_767 1_655 ?
O2 W1 Cs1 101.44(7) . 1_655 ?
O3 W1 Cs1 152.03(7) . 1_655 ?
O7 W1 Cs1 94.04(7) 3_767 1_655 ?
O1 W1 Cs1 130.357(6) . 1_655 ?
Nb3 W1 Cs1 85.409(6) 3_767 1_655 ?
O5 W1 Cs2 27.14(9) . 4_766 ?
O10 W1 Cs2 120.07(7) 3_767 4_766 ?
O2 W1 Cs2 120.09(7) . 4_766 ?
O3 W1 Cs2 83.34(7) . 4_766 ?
O7 W1 Cs2 83.27(7) 3_767 4_766 ?
O1 W1 Cs2 153.085(6) . 4_766 ?
Nb3 W1 Cs2 148.856(6) 3_767 4_766 ?
Cs1 W1 Cs2 69.282(5) 1_655 4_766 ?
O8 W2 O6 102.71(11) . . ?
O8 W2 O4 102.85(11) . . ?
O6 W2 O4 154.44(10) . . ?
O8 W2 O2 101.32(11) . . ?
O6 W2 O2 86.84(10) . . ?
O4 W2 O2 87.99(10) . . ?
O8 W2 O7 104.37(11) . . ?
O6 W2 O7 87.17(10) . . ?
O4 W2 O7 86.73(10) . . ?
O2 W2 O7 154.31(10) . . ?
O8 W2 O1 178.45(9) . . ?
O6 W2 O1 76.60(7) . . ?
O4 W2 O1 77.84(7) . . ?
O2 W2 O1 77.29(7) . . ?
O7 W2 O1 77.02(7) . . ?
O8 W2 Cs2 51.96(8) . 4_666 ?
O6 W2 Cs2 151.91(7) . 4_666 ?
O4 W2 Cs2 52.52(7) . 4_666 ?
O2 W2 Cs2 108.21(7) . 4_666 ?
O7 W2 Cs2 88.22(7) . 4_666 ?
O1 W2 Cs2 129.030(7) . 4_666 ?
O8 W2 Cs1 35.40(9) . . ?
O6 W2 Cs1 81.94(7) . . ?
O4 W2 Cs1 120.15(7) . . ?
O2 W2 Cs1 128.63(7) . . ?
O7 W2 Cs1 75.01(7) . . ?
O1 W2 Cs1 145.334(7) . . ?
Cs2 W2 Cs1 70.101(6) 4_666 . ?
O9 W3 O4 104.97(12) . . ?
O9 W3 O10 101.74(11) . . ?
O4 W3 O10 88.22(11) . . ?
O9 W3 O6 99.50(12) . 3_767 ?
O4 W3 O6 155.53(10) . 3_767 ?
O10 W3 O6 87.25(10) . 3_767 ?
O9 W3 O3 102.84(11) . . ?
O4 W3 O3 87.27(10) . . ?
O10 W3 O3 155.35(10) . . ?
O6 W3 O3 86.89(10) 3_767 . ?
O9 W3 O1 176.50(10) . . ?
O4 W3 O1 78.52(7) . . ?
O10 W3 O1 77.90(7) . . ?
O6 W3 O1 77.02(7) 3_767 . ?
O3 W3 O1 77.45(7) . . ?
O9 W3 Nb1 134.21(9) . 3_767 ?
O4 W3 Nb1 82.15(7) . 3_767 ?
O10 W3 Nb1 32.53(7) . 3_767 ?
O6 W3 Nb1 81.15(7) 3_767 3_767 ?
O3 W3 Nb1 122.82(7) . 3_767 ?
O1 W3 Nb1 45.370(5) . 3_767 ?
O9 W3 Cs2 63.29(10) . 3_667 ?
O4 W3 Cs2 140.57(7) . 3_667 ?
O10 W3 Cs2 60.56(7) . 3_667 ?
O6 W3 Cs2 53.74(7) 3_767 3_667 ?
O3 W3 Cs2 131.19(7) . 3_667 ?
O1 W3 Cs2 113.835(7) . 3_667 ?
Nb1 W3 Cs2 82.401(6) 3_767 3_667 ?
O9 W3 Cs1 72.18(10) . 4_666 ?
O4 W3 Cs1 54.91(7) . 4_666 ?
O10 W3 Cs1 137.10(7) . 4_666 ?
O6 W3 Cs1 135.48(7) 3_767 4_666 ?
O3 W3 Cs1 54.71(7) . 4_666 ?
O1 W3 Cs1 110.507(7) . 4_666 ?
Nb1 W3 Cs1 136.285(7) 3_767 4_666 ?
Cs2 W3 Cs1 135.285(7) 3_667 4_666 ?
O14 Cs1 O13 146.91(8) . . ?
O14 Cs1 O8 73.36(7) . . ?
O13 Cs1 O8 81.02(8) . . ?
O14 Cs1 O11 68.70(8) . . ?
O13 Cs1 O11 141.86(8) . . ?
O8 Cs1 O11 136.25(7) . . ?
O14 Cs1 O12 61.18(7) . . ?
O13 Cs1 O12 135.78(8) . . ?
O8 Cs1 O12 82.12(7) . . ?
O11 Cs1 O12 61.01(7) . . ?
O14 Cs1 O5 133.00(7) . 1_455 ?
O13 Cs1 O5 57.53(7) . 1_455 ?
O8 Cs1 O5 77.60(7) . 1_455 ?
O11 Cs1 O5 114.07(7) . 1_455 ?
O12 Cs1 O5 79.02(7) . 1_455 ?
O14 Cs1 O10 114.67(7) . 3_667 ?
O13 Cs1 O10 95.80(7) . 3_667 ?
O8 Cs1 O10 118.77(6) . 3_667 ?
O11 Cs1 O10 62.27(7) . 3_667 ?
O12 Cs1 O10 58.44(7) . 3_667 ?
O5 Cs1 O10 52.17(6) 1_455 3_667 ?
O14 Cs1 O3 72.36(7) . 4_565 ?
O13 Cs1 O3 87.80(7) . 4_565 ?
O8 Cs1 O3 91.06(6) . 4_565 ?
O11 Cs1 O3 97.40(7) . 4_565 ?
O12 Cs1 O3 133.10(7) . 4_565 ?
O5 Cs1 O3 144.59(6) 1_455 4_565 ?
O10 Cs1 O3 150.17(6) 3_667 4_565 ?
O14 Cs1 O4 100.86(7) . 4_565 ?
O13 Cs1 O4 83.72(8) . 4_565 ?
O8 Cs1 O4 136.93(6) . 4_565 ?
O11 Cs1 O4 72.54(7) . 4_565 ?
O12 Cs1 O4 133.48(7) . 4_565 ?
O5 Cs1 O4 125.34(6) 1_455 4_565 ?
O10 Cs1 O4 102.65(6) 3_667 4_565 ?
O3 Cs1 O4 48.19(6) 4_565 4_565 ?
O14 Cs1 Na1 37.03(6) . 2_556 ?
O13 Cs1 Na1 174.40(6) . 2_556 ?
O8 Cs1 Na1 99.18(5) . 2_556 ?
O11 Cs1 Na1 37.21(6) . 2_556 ?
O12 Cs1 Na1 39.14(6) . 2_556 ?
O5 Cs1 Na1 116.97(5) 1_455 2_556 ?
O10 Cs1 Na1 79.16(5) 3_667 2_556 ?
O3 Cs1 Na1 97.78(5) 4_565 2_556 ?
O4 Cs1 Na1 99.70(5) 4_565 2_556 ?
O14 Cs1 Nb3 99.62(6) . 4_565 ?
O13 Cs1 Nb3 68.93(6) . 4_565 ?
O8 Cs1 Nb3 108.63(5) . 4_565 ?
O11 Cs1 Nb3 98.56(5) . 4_565 ?
O12 Cs1 Nb3 155.18(5) . 4_565 ?
O5 Cs1 Nb3 124.57(5) 1_455 4_565 ?
O10 Cs1 Nb3 127.14(4) 3_667 4_565 ?
O3 Cs1 Nb3 29.02(4) 4_565 4_565 ?
O4 Cs1 Nb3 28.81(4) 4_565 4_565 ?
Na1 Cs1 Nb3 116.06(3) 2_556 4_565 ?
O14 Cs1 W3 99.62(6) . 4_565 ?
O13 Cs1 W3 68.93(6) . 4_565 ?
O8 Cs1 W3 108.63(5) . 4_565 ?
O11 Cs1 W3 98.56(5) . 4_565 ?
O12 Cs1 W3 155.18(5) . 4_565 ?
O5 Cs1 W3 124.57(5) 1_455 4_565 ?
O10 Cs1 W3 127.14(4) 3_667 4_565 ?
O3 Cs1 W3 29.02(4) 4_565 4_565 ?
O4 Cs1 W3 28.81(4) 4_565 4_565 ?
Na1 Cs1 W3 116.06(3) 2_556 4_565 ?
Nb3 Cs1 W3 0.000(2) 4_565 4_565 ?
O5 Cs2 O6 90.15(7) 4_465 1_455 ?
O5 Cs2 O12 72.78(7) 4_465 2_546 ?
O6 Cs2 O12 137.59(7) 1_455 2_546 ?
O5 Cs2 O16 71.25(7) 4_465 . ?
O6 Cs2 O16 74.16(7) 1_455 . ?
O12 Cs2 O16 63.68(8) 2_546 . ?
O5 Cs2 O4 115.08(7) 4_465 4_565 ?
O6 Cs2 O4 153.56(6) 1_455 4_565 ?
O12 Cs2 O4 62.78(7) 2_546 4_565 ?
O16 Cs2 O4 119.91(7) . 4_565 ?
O5 Cs2 O8 80.20(7) 4_465 4_565 ?
O6 Cs2 O8 129.01(6) 1_455 4_565 ?
O12 Cs2 O8 86.90(7) 2_546 4_565 ?
O16 Cs2 O8 143.62(7) . 4_565 ?
O4 Cs2 O8 53.87(6) 4_565 4_565 ?
O5 Cs2 O10 135.24(7) 4_465 3_667 ?
O6 Cs2 O10 49.60(6) 1_455 3_667 ?
O12 Cs2 O10 148.93(7) 2_546 3_667 ?
O16 Cs2 O10 107.73(7) . 3_667 ?
O4 Cs2 O10 104.02(6) 4_565 3_667 ?
O8 Cs2 O10 108.39(6) 4_565 3_667 ?
O5 Cs2 O15 126.38(7) 4_465 . ?
O6 Cs2 O15 85.44(7) 1_455 . ?
O12 Cs2 O15 75.34(7) 2_546 . ?
O16 Cs2 O15 56.15(8) . . ?
O4 Cs2 O15 85.52(7) 4_565 . ?
O8 Cs2 O15 139.28(7) 4_565 . ?
O10 Cs2 O15 75.66(6) 3_667 . ?
O5 Cs2 O9 90.98(7) 4_465 3_667 ?
O6 Cs2 O9 51.73(6) 1_455 3_667 ?
O12 Cs2 O9 159.76(7) 2_546 3_667 ?
O16 Cs2 O9 123.20(7) . 3_667 ?
O4 Cs2 O9 116.53(6) 4_565 3_667 ?
O8 Cs2 O9 78.29(6) 4_565 3_667 ?
O10 Cs2 O9 50.83(6) 3_667 3_667 ?
O15 Cs2 O9 124.79(6) . 3_667 ?
O5 Cs2 O11 116.27(7) 4_465 . ?
O6 Cs2 O11 93.15(7) 1_455 . ?
O12 Cs2 O11 129.26(7) 2_546 . ?
O16 Cs2 O11 165.67(7) . . ?
O4 Cs2 O11 69.30(7) 4_565 . ?
O8 Cs2 O11 50.30(7) 4_565 . ?
O10 Cs2 O11 58.12(6) 3_667 . ?
O15 Cs2 O11 117.32(7) . . ?
O9 Cs2 O11 47.52(7) 3_667 . ?
O5 Cs2 Na1 92.47(6) 4_465 . ?
O6 Cs2 Na1 104.91(5) 1_455 . ?
O12 Cs2 Na1 40.27(6) 2_546 . ?
O16 Cs2 Na1 37.75(6) . . ?
O4 Cs2 Na1 82.85(5) 4_565 . ?
O8 Cs2 Na1 125.28(5) 4_565 . ?
O10 Cs2 Na1 113.92(5) 3_667 . ?
O15 Cs2 Na1 38.83(6) . . ?
O9 Cs2 Na1 156.41(5) 3_667 . ?
O11 Cs2 Na1 146.14(6) . . ?
O5 Cs2 W3 104.67(5) 4_465 3_667 ?
O6 Cs2 W3 30.75(4) 1_455 3_667 ?
O12 Cs2 W3 168.15(5) 2_546 3_667 ?
O16 Cs2 W3 104.48(6) . 3_667 ?
O4 Cs2 W3 127.23(5) 4_565 3_667 ?
O8 Cs2 W3 104.21(5) 4_565 3_667 ?
O10 Cs2 W3 30.76(4) 3_667 3_667 ?
O15 Cs2 W3 98.03(5) . 3_667 ?
O9 Cs2 W3 27.65(4) 3_667 3_667 ?
O11 Cs2 W3 62.45(5) . 3_667 ?
Na1 Cs2 W3 129.80(3) . 3_667 ?
O16 Na1 O14 95.67(13) . 2_546 ?
O16 Na1 O11 164.10(14) . 2_546 ?
O14 Na1 O11 97.17(12) 2_546 2_546 ?
O16 Na1 O15 80.79(12) . . ?
O14 Na1 O15 167.13(14) 2_546 . ?
O11 Na1 O15 88.61(12) 2_546 . ?
O16 Na1 O12 87.60(12) . 2_546 ?
O14 Na1 O12 83.50(11) 2_546 2_546 ?
O11 Na1 O12 84.57(11) 2_546 2_546 ?
O15 Na1 O12 108.57(12) . 2_546 ?
O16 Na1 O15 107.62(13) . 3_557 ?
O14 Na1 O15 78.76(11) 2_546 3_557 ?
O11 Na1 O15 84.13(11) 2_546 3_557 ?
O15 Na1 O15 90.46(12) . 3_557 ?
O12 Na1 O15 157.57(12) 2_546 3_557 ?
O16 Na1 Na1 96.33(11) . 3_557 ?
O14 Na1 Na1 122.03(11) 2_546 3_557 ?
O11 Na1 Na1 84.76(10) 2_546 3_557 ?
O15 Na1 Na1 46.85(9) . 3_557 ?
O12 Na1 Na1 153.39(11) 2_546 3_557 ?
O15 Na1 Na1 43.61(8) 3_557 3_557 ?
O16 Na1 Cs2 56.43(10) . . ?
O14 Na1 Cs2 127.37(9) 2_546 . ?
O11 Na1 Cs2 107.97(9) 2_546 . ?
O15 Na1 Cs2 60.60(8) . . ?
O12 Na1 Cs2 54.95(8) 2_546 . ?
O15 Na1 Cs2 147.42(9) 3_557 . ?
Na1 Na1 Cs2 106.03(7) 3_557 . ?
O16 Na1 Cs1 129.84(10) . 2_546 ?
O14 Na1 Cs1 52.10(8) 2_546 2_546 ?
O11 Na1 Cs1 54.55(9) 2_546 2_546 ?
O15 Na1 Cs1 138.56(9) . 2_546 ?
O12 Na1 Cs1 55.51(8) 2_546 2_546 ?
O15 Na1 Cs1 102.34(8) 3_557 2_546 ?
Na1 Na1 Cs1 132.30(8) 3_557 2_546 ?
Cs2 Na1 Cs1 109.33(4) . 2_546 ?
Nb3 O1 W3 0.000(10) 3_767 3_767 ?
Nb3 O1 W3 180.0 3_767 . ?
W3 O1 W3 180.0 3_767 . ?
Nb3 O1 Nb1 90.410(6) 3_767 3_767 ?
W3 O1 Nb1 90.410(6) 3_767 3_767 ?
W3 O1 Nb1 89.590(6) . 3_767 ?
Nb3 O1 W1 90.410(6) 3_767 3_767 ?
W3 O1 W1 90.410(6) 3_767 3_767 ?
W3 O1 W1 89.590(6) . 3_767 ?
Nb1 O1 W1 0.000(5) 3_767 3_767 ?
Nb3 O1 W1 89.590(6) 3_767 . ?
W3 O1 W1 89.590(6) 3_767 . ?
W3 O1 W1 90.410(6) . . ?
Nb1 O1 W1 180.0 3_767 . ?
W1 O1 W1 180.0 3_767 . ?
Nb3 O1 W2 90.628(7) 3_767 . ?
W3 O1 W2 90.628(7) 3_767 . ?
W3 O1 W2 89.372(7) . . ?
Nb1 O1 W2 90.175(6) 3_767 . ?
W1 O1 W2 90.175(6) 3_767 . ?
W1 O1 W2 89.825(6) . . ?
Nb3 O1 W2 89.372(7) 3_767 3_767 ?
W3 O1 W2 89.372(7) 3_767 3_767 ?
W3 O1 W2 90.628(7) . 3_767 ?
Nb1 O1 W2 89.825(6) 3_767 3_767 ?
W1 O1 W2 89.825(6) 3_767 3_767 ?
W1 O1 W2 90.175(6) . 3_767 ?
W2 O1 W2 180.0 . 3_767 ?
Nb3 O1 Nb2 89.372(7) 3_767 3_767 ?
W3 O1 Nb2 89.372(7) 3_767 3_767 ?
W3 O1 Nb2 90.628(7) . 3_767 ?
Nb1 O1 Nb2 89.825(6) 3_767 3_767 ?
W1 O1 Nb2 89.825(6) 3_767 3_767 ?
W1 O1 Nb2 90.175(6) . 3_767 ?
W2 O1 Nb2 180.0 . 3_767 ?
W2 O1 Nb2 0.000(11) 3_767 3_767 ?
W1 O2 W2 115.14(12) . . ?
W1 O3 W3 114.80(11) . . ?
W1 O3 Cs1 119.54(10) . 4_666 ?
W3 O3 Cs1 96.27(8) . 4_666 ?
W3 O4 W2 114.27(11) . . ?
W3 O4 Cs2 145.03(11) . 4_666 ?
W2 O4 Cs2 98.53(9) . 4_666 ?
W3 O4 Cs1 96.28(9) . 4_666 ?
W2 O4 Cs1 118.79(10) . 4_666 ?
Cs2 O4 Cs1 77.01(5) 4_666 4_666 ?
W1 O5 Cs2 137.56(13) . 4_766 ?
W1 O5 Cs1 105.94(11) . 1_655 ?
Cs2 O5 Cs1 101.99(7) 4_766 1_655 ?
W2 O6 Nb3 115.75(11) . 3_767 ?
W2 O6 W3 115.75(11) . 3_767 ?
Nb3 O6 W3 0.000(13) 3_767 3_767 ?
W2 O6 Cs2 124.28(11) . 1_655 ?
Nb3 O6 Cs2 95.50(9) 3_767 1_655 ?
W3 O6 Cs2 95.50(9) 3_767 1_655 ?
Nb1 O7 W1 0.000(10) 3_767 3_767 ?
Nb1 O7 W2 115.21(11) 3_767 . ?
W1 O7 W2 115.21(11) 3_767 . ?
W2 O8 Cs1 125.79(12) . . ?
W2 O8 Cs2 102.47(10) . 4_666 ?
Cs1 O8 Cs2 98.91(7) . 4_666 ?
W3 O9 Cs2 89.05(10) . 3_667 ?
Nb1 O10 W1 0.000(9) 3_767 3_767 ?
Nb1 O10 W3 114.61(11) 3_767 . ?
W1 O10 W3 114.61(11) 3_767 . ?
Nb1 O10 Cs1 99.34(9) 3_767 3_667 ?
W1 O10 Cs1 99.34(9) 3_767 3_667 ?
W3 O10 Cs1 145.69(11) . 3_667 ?
Nb1 O10 Cs2 123.87(10) 3_767 3_667 ?
W1 O10 Cs2 123.87(10) 3_767 3_667 ?
W3 O10 Cs2 88.68(8) . 3_667 ?
Cs1 O10 Cs2 75.72(5) 3_667 3_667 ?
Na1 O11 Cs1 88.24(10) 2_556 . ?
Na1 O11 Cs2 160.53(14) 2_556 . ?
Cs1 O11 Cs2 74.16(7) . . ?
Na1 O12 Cs2 84.78(9) 2_556 2_556 ?
Na1 O12 Cs1 85.35(9) 2_556 . ?
Cs2 O12 Cs1 163.30(10) 2_556 . ?
Na1 O14 Cs1 90.87(10) 2_556 . ?
Na1 O15 Na1 89.54(12) . 3_557 ?
Na1 O15 Cs2 80.57(9) . . ?
Na1 O15 Cs2 161.50(12) 3_557 . ?
Na1 O16 Cs2 85.83(11) . . ?



loop_

_geom_torsion_atom_site_label_1

_geom_torsion_atom_site_label_2

_geom_torsion_atom_site_label_3

_geom_torsion_atom_site_label_4

_geom_torsion

_geom_torsion_site_symmetry_1

_geom_torsion_site_symmetry_2

_geom_torsion_site_symmetry_3

_geom_torsion_site_symmetry_4

_geom_torsion_publ_flag


























































































































































































































































































































































































































































































































































































































O5 Cs2 Na1 O16 -54.46(11) 4_465 . . . ?
O6 Cs2 Na1 O16 36.35(11) 1_455 . . . ?
O12 Cs2 Na1 O16 -113.84(13) 2_546 . . . ?
O4 Cs2 Na1 O16 -169.44(11) 4_565 . . . ?
O8 Cs2 Na1 O16 -134.19(11) 4_565 . . . ?
O10 Cs2 Na1 O16 88.35(10) 3_667 . . . ?
O15 Cs2 Na1 O16 98.82(13) . . . . ?
O9 Cs2 Na1 O16 43.67(17) 3_667 . . . ?
O11 Cs2 Na1 O16 156.29(13) . . . . ?
W3 Cs2 Na1 O16 57.00(10) 3_667 . . . ?
O5 Cs2 Na1 O14 14.58(13) 4_465 . . 2_546 ?
O6 Cs2 Na1 O14 105.39(13) 1_455 . . 2_546 ?
O12 Cs2 Na1 O14 -44.80(14) 2_546 . . 2_546 ?
O16 Cs2 Na1 O14 69.05(15) . . . 2_546 ?
O4 Cs2 Na1 O14 -100.39(13) 4_565 . . 2_546 ?
O8 Cs2 Na1 O14 -65.15(14) 4_565 . . 2_546 ?
O10 Cs2 Na1 O14 157.40(12) 3_667 . . 2_546 ?
O15 Cs2 Na1 O14 167.87(16) . . . 2_546 ?
O9 Cs2 Na1 O14 112.71(17) 3_667 . . 2_546 ?
O11 Cs2 Na1 O14 -134.67(14) . . . 2_546 ?
W3 Cs2 Na1 O14 126.05(12) 3_667 . . 2_546 ?
O5 Cs2 Na1 O11 128.96(11) 4_465 . . 2_546 ?
O6 Cs2 Na1 O11 -140.23(11) 1_455 . . 2_546 ?
O12 Cs2 Na1 O11 69.58(13) 2_546 . . 2_546 ?
O16 Cs2 Na1 O11 -176.58(15) . . . 2_546 ?
O4 Cs2 Na1 O11 13.98(11) 4_565 . . 2_546 ?
O8 Cs2 Na1 O11 49.23(12) 4_565 . . 2_546 ?
O10 Cs2 Na1 O11 -88.23(11) 3_667 . . 2_546 ?
O15 Cs2 Na1 O11 -77.76(13) . . . 2_546 ?
O9 Cs2 Na1 O11 -132.91(15) 3_667 . . 2_546 ?
O11 Cs2 Na1 O11 -20.29(18) . . . 2_546 ?
W3 Cs2 Na1 O11 -119.58(10) 3_667 . . 2_546 ?
O5 Cs2 Na1 O15 -153.29(10) 4_465 . . . ?
O6 Cs2 Na1 O15 -62.48(10) 1_455 . . . ?
O12 Cs2 Na1 O15 147.33(13) 2_546 . . . ?
O16 Cs2 Na1 O15 -98.82(13) . . . . ?
O4 Cs2 Na1 O15 91.74(10) 4_565 . . . ?
O8 Cs2 Na1 O15 126.98(10) 4_565 . . . ?
O10 Cs2 Na1 O15 -10.47(10) 3_667 . . . ?
O9 Cs2 Na1 O15 -55.16(16) 3_667 . . . ?
O11 Cs2 Na1 O15 57.46(13) . . . . ?
W3 Cs2 Na1 O15 -41.82(10) 3_667 . . . ?
O5 Cs2 Na1 O12 59.38(10) 4_465 . . 2_546 ?
O6 Cs2 Na1 O12 150.19(9) 1_455 . . 2_546 ?
O16 Cs2 Na1 O12 113.84(13) . . . 2_546 ?
O4 Cs2 Na1 O12 -55.59(9) 4_565 . . 2_546 ?
O8 Cs2 Na1 O12 -20.35(11) 4_565 . . 2_546 ?
O10 Cs2 Na1 O12 -157.80(9) 3_667 . . 2_546 ?
O15 Cs2 Na1 O12 -147.33(13) . . . 2_546 ?
O9 Cs2 Na1 O12 157.51(14) 3_667 . . 2_546 ?
O11 Cs2 Na1 O12 -89.87(13) . . . 2_546 ?
W3 Cs2 Na1 O12 170.84(8) 3_667 . . 2_546 ?
O5 Cs2 Na1 O15 -123.12(17) 4_465 . . 3_557 ?
O6 Cs2 Na1 O15 -32.31(18) 1_455 . . 3_557 ?
O12 Cs2 Na1 O15 177.5(2) 2_546 . . 3_557 ?
O16 Cs2 Na1 O15 -68.65(19) . . . 3_557 ?
O4 Cs2 Na1 O15 121.91(17) 4_565 . . 3_557 ?
O8 Cs2 Na1 O15 157.15(17) 4_565 . . 3_557 ?
O10 Cs2 Na1 O15 19.70(18) 3_667 . . 3_557 ?
O15 Cs2 Na1 O15 30.2(2) . . . 3_557 ?
O9 Cs2 Na1 O15 -25.0(2) 3_667 . . 3_557 ?
O11 Cs2 Na1 O15 87.63(19) . . . 3_557 ?
W3 Cs2 Na1 O15 -11.65(18) 3_667 . . 3_557 ?
O5 Cs2 Na1 Na1 -141.43(8) 4_465 . . 3_557 ?
O6 Cs2 Na1 Na1 -50.62(8) 1_455 . . 3_557 ?
O12 Cs2 Na1 Na1 159.19(12) 2_546 . . 3_557 ?
O16 Cs2 Na1 Na1 -86.97(12) . . . 3_557 ?
O4 Cs2 Na1 Na1 103.59(8) 4_565 . . 3_557 ?
O8 Cs2 Na1 Na1 138.84(8) 4_565 . . 3_557 ?
O10 Cs2 Na1 Na1 1.38(9) 3_667 . . 3_557 ?
O15 Cs2 Na1 Na1 11.85(9) . . . 3_557 ?
O9 Cs2 Na1 Na1 -43.30(16) 3_667 . . 3_557 ?
O11 Cs2 Na1 Na1 69.32(12) . . . 3_557 ?
W3 Cs2 Na1 Na1 -29.97(8) 3_667 . . 3_557 ?
O5 Cs2 Na1 Cs1 71.13(6) 4_465 . . 2_546 ?
O6 Cs2 Na1 Cs1 161.94(5) 1_455 . . 2_546 ?
O12 Cs2 Na1 Cs1 11.75(8) 2_546 . . 2_546 ?
O16 Cs2 Na1 Cs1 125.59(11) . . . 2_546 ?
O4 Cs2 Na1 Cs1 -43.84(6) 4_565 . . 2_546 ?
O8 Cs2 Na1 Cs1 -8.60(8) 4_565 . . 2_546 ?
O10 Cs2 Na1 Cs1 -146.05(5) 3_667 . . 2_546 ?
O15 Cs2 Na1 Cs1 -135.58(10) . . . 2_546 ?
O9 Cs2 Na1 Cs1 169.26(12) 3_667 . . 2_546 ?
O11 Cs2 Na1 Cs1 -78.12(10) . . . 2_546 ?
W3 Cs2 Na1 Cs1 -177.407(16) 3_667 . . 2_546 ?
O9 W3 O1 Nb3 -126.7(15) . . . 3_767 ?
O4 W3 O1 Nb3 48.34(11) . . . 3_767 ?
O10 W3 O1 Nb3 -42.30(12) . . . 3_767 ?
O6 W3 O1 Nb3 -132.25(12) 3_767 . . 3_767 ?
O3 W3 O1 Nb3 138.08(11) . . . 3_767 ?
Nb1 W3 O1 Nb3 -41.93(9) 3_767 . . 3_767 ?
Cs2 W3 O1 Nb3 -92.19(9) 3_667 . . 3_767 ?
Cs1 W3 O1 Nb3 93.73(9) 4_666 . . 3_767 ?
O9 W3 O1 W3 -126.7(15) . . . 3_767 ?
O4 W3 O1 W3 48.34(11) . . . 3_767 ?
O10 W3 O1 W3 -42.30(12) . . . 3_767 ?
O6 W3 O1 W3 -132.25(12) 3_767 . . 3_767 ?
O3 W3 O1 W3 138.08(11) . . . 3_767 ?
Nb1 W3 O1 W3 -41.93(9) 3_767 . . 3_767 ?
Cs2 W3 O1 W3 -92.19(9) 3_667 . . 3_767 ?
Cs1 W3 O1 W3 93.73(9) 4_666 . . 3_767 ?
O9 W3 O1 Nb1 -84.8(15) . . . 3_767 ?
O4 W3 O1 Nb1 90.26(8) . . . 3_767 ?
O10 W3 O1 Nb1 -0.38(7) . . . 3_767 ?
O6 W3 O1 Nb1 -90.32(8) 3_767 . . 3_767 ?
O3 W3 O1 Nb1 180.00(7) . . . 3_767 ?
Cs2 W3 O1 Nb1 -50.262(8) 3_667 . . 3_767 ?
Cs1 W3 O1 Nb1 135.655(7) 4_666 . . 3_767 ?
O9 W3 O1 W1 -84.8(15) . . . 3_767 ?
O4 W3 O1 W1 90.26(8) . . . 3_767 ?
O10 W3 O1 W1 -0.38(7) . . . 3_767 ?
O6 W3 O1 W1 -90.32(8) 3_767 . . 3_767 ?
O3 W3 O1 W1 180.00(7) . . . 3_767 ?
Nb1 W3 O1 W1 0.0 3_767 . . 3_767 ?
Cs2 W3 O1 W1 -50.262(8) 3_667 . . 3_767 ?
Cs1 W3 O1 W1 135.655(7) 4_666 . . 3_767 ?
O9 W3 O1 W1 95.2(15) . . . . ?
O4 W3 O1 W1 -89.74(8) . . . . ?
O10 W3 O1 W1 179.62(7) . . . . ?
O6 W3 O1 W1 89.68(8) 3_767 . . . ?
O3 W3 O1 W1 0.00(7) . . . . ?
Nb1 W3 O1 W1 180.0 3_767 . . . ?
Cs2 W3 O1 W1 129.738(8) 3_667 . . . ?
Cs1 W3 O1 W1 -44.345(7) 4_666 . . . ?
O9 W3 O1 W2 -175.0(15) . . . . ?
O4 W3 O1 W2 0.08(8) . . . . ?
O10 W3 O1 W2 -90.56(7) . . . . ?
O6 W3 O1 W2 179.50(8) 3_767 . . . ?
O3 W3 O1 W2 89.82(7) . . . . ?
Nb1 W3 O1 W2 -90.180(6) 3_767 . . . ?
Cs2 W3 O1 W2 -140.442(8) 3_667 . . . ?
Cs1 W3 O1 W2 45.475(7) 4_666 . . . ?
O9 W3 O1 W2 5.0(15) . . . 3_767 ?
O4 W3 O1 W2 -179.92(8) . . . 3_767 ?
O10 W3 O1 W2 89.44(7) . . . 3_767 ?
O6 W3 O1 W2 -0.50(8) 3_767 . . 3_767 ?
O3 W3 O1 W2 -90.18(7) . . . 3_767 ?
Nb1 W3 O1 W2 89.820(6) 3_767 . . 3_767 ?
Cs2 W3 O1 W2 39.558(8) 3_667 . . 3_767 ?
Cs1 W3 O1 W2 -134.525(7) 4_666 . . 3_767 ?
O9 W3 O1 Nb2 5.0(15) . . . 3_767 ?
O4 W3 O1 Nb2 -179.92(8) . . . 3_767 ?
O10 W3 O1 Nb2 89.44(7) . . . 3_767 ?
O6 W3 O1 Nb2 -0.50(8) 3_767 . . 3_767 ?
O3 W3 O1 Nb2 -90.18(7) . . . 3_767 ?
Nb1 W3 O1 Nb2 89.820(6) 3_767 . . 3_767 ?
Cs2 W3 O1 Nb2 39.558(8) 3_667 . . 3_767 ?
Cs1 W3 O1 Nb2 -134.525(7) 4_666 . . 3_767 ?
O5 W1 O1 Nb3 -107(11) . . . 3_767 ?
O10 W1 O1 Nb3 -0.38(7) 3_767 . . 3_767 ?
O2 W1 O1 Nb3 -90.28(7) . . . 3_767 ?
O3 W1 O1 Nb3 180.00(7) . . . 3_767 ?
O7 W1 O1 Nb3 89.11(7) 3_767 . . 3_767 ?
Cs1 W1 O1 Nb3 4.407(9) 1_655 . . 3_767 ?
Cs2 W1 O1 Nb3 134.825(14) 4_766 . . 3_767 ?
O5 W1 O1 W3 -107(11) . . . 3_767 ?
O10 W1 O1 W3 -0.38(7) 3_767 . . 3_767 ?
O2 W1 O1 W3 -90.28(7) . . . 3_767 ?
O3 W1 O1 W3 180.00(7) . . . 3_767 ?
O7 W1 O1 W3 89.11(7) 3_767 . . 3_767 ?
Nb3 W1 O1 W3 0.0 3_767 . . 3_767 ?
Cs1 W1 O1 W3 4.407(9) 1_655 . . 3_767 ?
Cs2 W1 O1 W3 134.825(14) 4_766 . . 3_767 ?
O5 W1 O1 W3 73(11) . . . . ?
O10 W1 O1 W3 179.62(7) 3_767 . . . ?
O2 W1 O1 W3 89.72(7) . . . . ?
O3 W1 O1 W3 0.00(7) . . . . ?
O7 W1 O1 W3 -90.89(7) 3_767 . . . ?
Nb3 W1 O1 W3 180.0 3_767 . . . ?
Cs1 W1 O1 W3 -175.593(9) 1_655 . . . ?
Cs2 W1 O1 W3 -45.175(14) 4_766 . . . ?
O5 W1 O1 Nb1 -23(100) . . . 3_767 ?
O10 W1 O1 Nb1 83(100) 3_767 . . 3_767 ?
O2 W1 O1 Nb1 -6(100) . . . 3_767 ?
O3 W1 O1 Nb1 -96(100) . . . 3_767 ?
O7 W1 O1 Nb1 173(100) 3_767 . . 3_767 ?
Nb3 W1 O1 Nb1 84(100) 3_767 . . 3_767 ?
Cs1 W1 O1 Nb1 88(100) 1_655 . . 3_767 ?
Cs2 W1 O1 Nb1 -141(100) 4_766 . . 3_767 ?
O5 W1 O1 W1 -23(100) . . . 3_767 ?
O10 W1 O1 W1 83(100) 3_767 . . 3_767 ?
O2 W1 O1 W1 -6(100) . . . 3_767 ?
O3 W1 O1 W1 -96(100) . . . 3_767 ?
O7 W1 O1 W1 173(100) 3_767 . . 3_767 ?
Nb3 W1 O1 W1 84(100) 3_767 . . 3_767 ?
Cs1 W1 O1 W1 88(100) 1_655 . . 3_767 ?
Cs2 W1 O1 W1 -141(100) 4_766 . . 3_767 ?
O5 W1 O1 W2 -17(11) . . . . ?
O10 W1 O1 W2 90.25(7) 3_767 . . . ?
O2 W1 O1 W2 0.35(7) . . . . ?
O3 W1 O1 W2 -89.37(7) . . . . ?
O7 W1 O1 W2 179.74(7) 3_767 . . . ?
Nb3 W1 O1 W2 90.629(7) 3_767 . . . ?
Cs1 W1 O1 W2 95.036(9) 1_655 . . . ?
Cs2 W1 O1 W2 -134.546(14) 4_766 . . . ?
O5 W1 O1 W2 163(21) . . . 3_767 ?
O10 W1 O1 W2 -89.75(7) 3_767 . . 3_767 ?
O2 W1 O1 W2 -179.65(7) . . . 3_767 ?
O3 W1 O1 W2 90.63(7) . . . 3_767 ?
O7 W1 O1 W2 -0.26(7) 3_767 . . 3_767 ?
Nb3 W1 O1 W2 -89.371(7) 3_767 . . 3_767 ?
Cs1 W1 O1 W2 -84.964(9) 1_655 . . 3_767 ?
Cs2 W1 O1 W2 45.454(14) 4_766 . . 3_767 ?
O5 W1 O1 Nb2 163(21) . . . 3_767 ?
O10 W1 O1 Nb2 -89.75(7) 3_767 . . 3_767 ?
O2 W1 O1 Nb2 -179.65(7) . . . 3_767 ?
O3 W1 O1 Nb2 90.63(7) . . . 3_767 ?
O7 W1 O1 Nb2 -0.26(7) 3_767 . . 3_767 ?
Nb3 W1 O1 Nb2 -89.371(7) 3_767 . . 3_767 ?
Cs1 W1 O1 Nb2 -84.964(9) 1_655 . . 3_767 ?
Cs2 W1 O1 Nb2 45.454(14) 4_766 . . 3_767 ?
O8 W2 O1 Nb3 63(3) . . . 3_767 ?
O6 W2 O1 Nb3 -0.51(8) . . . 3_767 ?
O4 W2 O1 Nb3 179.92(8) . . . 3_767 ?
O2 W2 O1 Nb3 89.24(7) . . . 3_767 ?
O7 W2 O1 Nb3 -90.67(7) . . . 3_767 ?
Cs2 W2 O1 Nb3 -167.493(9) 4_666 . . 3_767 ?
Cs1 W2 O1 Nb3 -53.797(13) . . . 3_767 ?
O8 W2 O1 W3 63(3) . . . 3_767 ?
O6 W2 O1 W3 -0.51(8) . . . 3_767 ?
O4 W2 O1 W3 179.92(8) . . . 3_767 ?
O2 W2 O1 W3 89.24(7) . . . 3_767 ?
O7 W2 O1 W3 -90.67(7) . . . 3_767 ?
Cs2 W2 O1 W3 -167.493(9) 4_666 . . 3_767 ?
Cs1 W2 O1 W3 -53.797(13) . . . 3_767 ?
O8 W2 O1 W3 -117(3) . . . . ?
O6 W2 O1 W3 179.49(8) . . . . ?
O4 W2 O1 W3 -0.08(8) . . . . ?
O2 W2 O1 W3 -90.76(7) . . . . ?
O7 W2 O1 W3 89.33(7) . . . . ?
Cs2 W2 O1 W3 12.507(9) 4_666 . . . ?
Cs1 W2 O1 W3 126.203(13) . . . . ?
O8 W2 O1 Nb1 154(3) . . . 3_767 ?
O6 W2 O1 Nb1 89.90(8) . . . 3_767 ?
O4 W2 O1 Nb1 -89.67(8) . . . 3_767 ?
O2 W2 O1 Nb1 179.65(7) . . . 3_767 ?
O7 W2 O1 Nb1 -0.26(7) . . . 3_767 ?
Cs2 W2 O1 Nb1 -77.081(9) 4_666 . . 3_767 ?
Cs1 W2 O1 Nb1 36.615(12) . . . 3_767 ?
O8 W2 O1 W1 154(3) . . . 3_767 ?
O6 W2 O1 W1 89.90(8) . . . 3_767 ?
O4 W2 O1 W1 -89.67(8) . . . 3_767 ?
O2 W2 O1 W1 179.65(7) . . . 3_767 ?
O7 W2 O1 W1 -0.26(7) . . . 3_767 ?
Cs2 W2 O1 W1 -77.081(9) 4_666 . . 3_767 ?
Cs1 W2 O1 W1 36.615(12) . . . 3_767 ?
O8 W2 O1 W1 -26(3) . . . . ?
O6 W2 O1 W1 -90.10(8) . . . . ?
O4 W2 O1 W1 90.33(8) . . . . ?
O2 W2 O1 W1 -0.35(7) . . . . ?
O7 W2 O1 W1 179.74(7) . . . . ?
Cs2 W2 O1 W1 102.919(9) 4_666 . . . ?
Cs1 W2 O1 W1 -143.385(12) . . . . ?
O8 W2 O1 W2 162(100) . . . 3_767 ?
O6 W2 O1 W2 98(100) . . . 3_767 ?
O4 W2 O1 W2 -82(100) . . . 3_767 ?
O2 W2 O1 W2 -173(100) . . . 3_767 ?
O7 W2 O1 W2 8(100) . . . 3_767 ?
Cs2 W2 O1 W2 -69(100) 4_666 . . 3_767 ?
Cs1 W2 O1 W2 44(100) . . . 3_767 ?
O8 W2 O1 Nb2 162(100) . . . 3_767 ?
O6 W2 O1 Nb2 98(100) . . . 3_767 ?
O4 W2 O1 Nb2 -82(100) . . . 3_767 ?
O2 W2 O1 Nb2 -173(100) . . . 3_767 ?
O7 W2 O1 Nb2 8(100) . . . 3_767 ?
Cs2 W2 O1 Nb2 -69(100) 4_666 . . 3_767 ?
Cs1 W2 O1 Nb2 44(100) . . . 3_767 ?
O5 W1 O2 W2 179.40(13) . . . . ?
O10 W1 O2 W2 -78.64(13) 3_767 . . . ?
O3 W1 O2 W2 77.22(13) . . . . ?
O7 W1 O2 W2 -1.9(3) 3_767 . . . ?
O1 W1 O2 W2 -0.46(10) . . . . ?
Nb3 W1 O2 W2 -46.13(10) 3_767 . . . ?
Cs1 W1 O2 W2 -129.67(10) 1_655 . . . ?
Cs2 W1 O2 W2 157.79(7) 4_766 . . . ?
O8 W2 O2 W1 179.77(13) . . . . ?
O6 W2 O2 W1 77.43(13) . . . . ?
O4 W2 O2 W1 -77.53(13) . . . . ?
O7 W2 O2 W1 0.7(3) . . . . ?
O1 W2 O2 W1 0.46(9) . . . . ?
Cs2 W2 O2 W1 -126.80(10) 4_666 . . . ?
Cs1 W2 O2 W1 154.49(6) . . . . ?
O5 W1 O3 W3 -179.54(13) . . . . ?
O10 W1 O3 W3 -0.9(3) 3_767 . . . ?
O2 W1 O3 W3 -78.10(13) . . . . ?
O7 W1 O3 W3 77.70(13) 3_767 . . . ?
O1 W1 O3 W3 0.00(10) . . . . ?
Nb3 W1 O3 W3 0.00(16) 3_767 . . . ?
Cs1 W1 O3 W3 172.83(3) 1_655 . . . ?
Cs2 W1 O3 W3 161.14(12) 4_766 . . . ?
O5 W1 O3 Cs1 -65.95(13) . . . 4_666 ?
O10 W1 O3 Cs1 112.7(2) 3_767 . . 4_666 ?
O2 W1 O3 Cs1 35.49(11) . . . 4_666 ?
O7 W1 O3 Cs1 -168.71(11) 3_767 . . 4_666 ?
O1 W1 O3 Cs1 113.59(9) . . . 4_666 ?
Nb3 W1 O3 Cs1 113.59(8) 3_767 . . 4_666 ?
Cs1 W1 O3 Cs1 -73.59(18) 1_655 . . 4_666 ?
Cs2 W1 O3 Cs1 -85.27(8) 4_766 . . 4_666 ?
O9 W3 O3 W1 -176.42(13) . . . . ?
O4 W3 O3 W1 78.84(13) . . . . ?
O10 W3 O3 W1 -0.9(3) . . . . ?
O6 W3 O3 W1 -77.38(13) 3_767 . . . ?
O1 W3 O3 W1 0.00(10) . . . . ?
Nb1 W3 O3 W1 0.00(16) 3_767 . . . ?
Cs2 W3 O3 W1 -110.82(11) 3_667 . . . ?
Cs1 W3 O3 W1 126.67(15) 4_666 . . . ?
O9 W3 O3 Cs1 56.91(11) . . . 4_666 ?
O4 W3 O3 Cs1 -47.83(8) . . . 4_666 ?
O10 W3 O3 Cs1 -127.6(2) . . . 4_666 ?
O6 W3 O3 Cs1 155.95(8) 3_767 . . 4_666 ?
O1 W3 O3 Cs1 -126.67(6) . . . 4_666 ?
Nb1 W3 O3 Cs1 -126.67(4) 3_767 . . 4_666 ?
Cs2 W3 O3 Cs1 122.51(6) 3_667 . . 4_666 ?
O9 W3 O4 W2 179.58(13) . . . . ?
O10 W3 O4 W2 77.91(14) . . . . ?
O6 W3 O4 W2 -1.5(3) 3_767 . . . ?
O3 W3 O4 W2 -77.85(13) . . . . ?
O1 W3 O4 W2 -0.11(10) . . . . ?
Nb1 W3 O4 W2 45.81(11) 3_767 . . . ?
Cs2 W3 O4 W2 113.61(11) 3_667 . . . ?
Cs1 W3 O4 W2 -125.53(15) 4_666 . . . ?
O9 W3 O4 Cs2 21.4(2) . . . 4_666 ?
O10 W3 O4 Cs2 -80.3(2) . . . 4_666 ?
O6 W3 O4 Cs2 -159.69(19) 3_767 . . 4_666 ?
O3 W3 O4 Cs2 123.9(2) . . . 4_666 ?
O1 W3 O4 Cs2 -158.3(2) . . . 4_666 ?
Nb1 W3 O4 Cs2 -112.39(19) 3_767 . . 4_666 ?
Cs2 W3 O4 Cs2 -44.6(3) 3_667 . . 4_666 ?
Cs1 W3 O4 Cs2 76.27(18) 4_666 . . 4_666 ?
O9 W3 O4 Cs1 -54.89(11) . . . 4_666 ?
O10 W3 O4 Cs1 -156.57(8) . . . 4_666 ?
O6 W3 O4 Cs1 124.0(2) 3_767 . . 4_666 ?
O3 W3 O4 Cs1 47.67(8) . . . 4_666 ?
O1 W3 O4 Cs1 125.42(6) . . . 4_666 ?
Nb1 W3 O4 Cs1 171.34(6) 3_767 . . 4_666 ?
Cs2 W3 O4 Cs1 -120.86(8) 3_667 . . 4_666 ?
O8 W2 O4 W3 178.69(13) . . . . ?
O6 W2 O4 W3 -0.9(3) . . . . ?
O2 W2 O4 W3 77.53(14) . . . . ?
O7 W2 O4 W3 -77.31(14) . . . . ?
O1 W2 O4 W3 0.11(10) . . . . ?
Cs2 W2 O4 W3 -167.57(17) 4_666 . . . ?
Cs1 W2 O4 W3 -147.87(8) . . . . ?
O8 W2 O4 Cs2 -13.74(12) . . . 4_666 ?
O6 W2 O4 Cs2 166.7(2) . . . 4_666 ?
O2 W2 O4 Cs2 -114.89(9) . . . 4_666 ?
O7 W2 O4 Cs2 90.26(9) . . . 4_666 ?
O1 W2 O4 Cs2 167.68(7) . . . 4_666 ?
Cs1 W2 O4 Cs2 19.70(10) . . . 4_666 ?
O8 W2 O4 Cs1 66.07(13) . . . 4_666 ?
O6 W2 O4 Cs1 -113.5(2) . . . 4_666 ?
O2 W2 O4 Cs1 -35.09(11) . . . 4_666 ?
O7 W2 O4 Cs1 170.07(11) . . . 4_666 ?
O1 W2 O4 Cs1 -112.51(9) . . . 4_666 ?
Cs2 W2 O4 Cs1 79.81(9) 4_666 . . 4_666 ?
Cs1 W2 O4 Cs1 99.51(9) . . . 4_666 ?
O10 W1 O5 Cs2 134.49(18) 3_767 . . 4_766 ?
O2 W1 O5 Cs2 -135.68(18) . . . 4_766 ?
O3 W1 O5 Cs2 -46.1(2) . . . 4_766 ?
O7 W1 O5 Cs2 44.9(2) 3_767 . . 4_766 ?
O1 W1 O5 Cs2 -119(11) . . . 4_766 ?
Nb3 W1 O5 Cs2 134.46(13) 3_767 . . 4_766 ?
Cs1 W1 O5 Cs2 129.2(2) 1_655 . . 4_766 ?
O10 W1 O5 Cs1 5.26(12) 3_767 . . 1_655 ?
O2 W1 O5 Cs1 95.09(11) . . . 1_655 ?
O3 W1 O5 Cs1 -175.32(9) . . . 1_655 ?
O7 W1 O5 Cs1 -84.36(11) 3_767 . . 1_655 ?
O1 W1 O5 Cs1 112(11) . . . 1_655 ?
Nb3 W1 O5 Cs1 5.23(17) 3_767 . . 1_655 ?
Cs2 W1 O5 Cs1 -129.2(2) 4_766 . . 1_655 ?
O8 W2 O6 Nb3 -177.91(13) . . . 3_767 ?
O4 W2 O6 Nb3 1.6(3) . . . 3_767 ?
O2 W2 O6 Nb3 -77.01(14) . . . 3_767 ?
O7 W2 O6 Nb3 77.99(13) . . . 3_767 ?
O1 W2 O6 Nb3 0.67(10) . . . 3_767 ?
Cs2 W2 O6 Nb3 158.86(5) 4_666 . . 3_767 ?
Cs1 W2 O6 Nb3 153.24(13) . . . 3_767 ?
O8 W2 O6 W3 -177.91(13) . . . 3_767 ?
O4 W2 O6 W3 1.6(3) . . . 3_767 ?
O2 W2 O6 W3 -77.01(14) . . . 3_767 ?
O7 W2 O6 W3 77.99(13) . . . 3_767 ?
O1 W2 O6 W3 0.67(10) . . . 3_767 ?
Cs2 W2 O6 W3 158.86(5) 4_666 . . 3_767 ?
Cs1 W2 O6 W3 153.24(13) . . . 3_767 ?
O8 W2 O6 Cs2 -60.67(14) . . . 1_655 ?
O4 W2 O6 Cs2 118.9(2) . . . 1_655 ?
O2 W2 O6 Cs2 40.23(12) . . . 1_655 ?
O7 W2 O6 Cs2 -164.77(12) . . . 1_655 ?
O1 W2 O6 Cs2 117.90(11) . . . 1_655 ?
Cs2 W2 O6 Cs2 -83.90(18) 4_666 . . 1_655 ?
Cs1 W2 O6 Cs2 -89.52(10) . . . 1_655 ?
O8 W2 O7 Nb1 -178.96(13) . . . 3_767 ?
O6 W2 O7 Nb1 -76.56(13) . . . 3_767 ?
O4 W2 O7 Nb1 78.61(13) . . . 3_767 ?
O2 W2 O7 Nb1 0.1(3) . . . 3_767 ?
O1 W2 O7 Nb1 0.34(9) . . . 3_767 ?
Cs2 W2 O7 Nb1 131.16(11) 4_666 . . 3_767 ?
Cs1 W2 O7 Nb1 -158.97(13) . . . 3_767 ?
O8 W2 O7 W1 -178.96(13) . . . 3_767 ?
O6 W2 O7 W1 -76.56(13) . . . 3_767 ?
O4 W2 O7 W1 78.61(13) . . . 3_767 ?
O2 W2 O7 W1 0.1(3) . . . 3_767 ?
O1 W2 O7 W1 0.34(9) . . . 3_767 ?
Cs2 W2 O7 W1 131.16(11) 4_666 . . 3_767 ?
Cs1 W2 O7 W1 -158.97(13) . . . 3_767 ?
O6 W2 O8 Cs1 -55.56(15) . . . . ?
O4 W2 O8 Cs1 124.65(13) . . . . ?
O2 W2 O8 Cs1 -144.84(13) . . . . ?
O7 W2 O8 Cs1 34.76(16) . . . . ?
O1 W2 O8 Cs1 -119(3) . . . . ?
Cs2 W2 O8 Cs1 110.80(16) 4_666 . . . ?
O6 W2 O8 Cs2 -166.36(9) . . . 4_666 ?
O4 W2 O8 Cs2 13.85(12) . . . 4_666 ?
O2 W2 O8 Cs2 104.36(10) . . . 4_666 ?
O7 W2 O8 Cs2 -76.04(10) . . . 4_666 ?
O1 W2 O8 Cs2 130(3) . . . 4_666 ?
Cs1 W2 O8 Cs2 -110.80(16) . . . 4_666 ?
O14 Cs1 O8 W2 38.37(14) . . . . ?
O13 Cs1 O8 W2 -162.80(16) . . . . ?
O11 Cs1 O8 W2 7.7(2) . . . . ?
O12 Cs1 O8 W2 -23.82(14) . . . . ?
O5 Cs1 O8 W2 -104.24(15) 1_455 . . . ?
O10 Cs1 O8 W2 -71.08(16) 3_667 . . . ?
O3 Cs1 O8 W2 109.60(15) 4_565 . . . ?
O4 Cs1 O8 W2 126.54(13) 4_565 . . . ?
Na1 Cs1 O8 W2 11.54(15) 2_556 . . . ?
Nb3 Cs1 O8 W2 133.14(13) 4_565 . . . ?
W3 Cs1 O8 W2 133.14(13) 4_565 . . . ?
O14 Cs1 O8 Cs2 150.86(9) . . . 4_666 ?
O13 Cs1 O8 Cs2 -50.30(8) . . . 4_666 ?
O11 Cs1 O8 Cs2 120.22(9) . . . 4_666 ?
O12 Cs1 O8 Cs2 88.67(8) . . . 4_666 ?
O5 Cs1 O8 Cs2 8.25(7) 1_455 . . 4_666 ?
O10 Cs1 O8 Cs2 41.42(9) 3_667 . . 4_666 ?
O3 Cs1 O8 Cs2 -137.91(7) 4_565 . . 4_666 ?
O4 Cs1 O8 Cs2 -120.96(8) 4_565 . . 4_666 ?
Na1 Cs1 O8 Cs2 124.03(6) 2_556 . . 4_666 ?
Nb3 Cs1 O8 Cs2 -114.36(5) 4_565 . . 4_666 ?
W3 Cs1 O8 Cs2 -114.36(5) 4_565 . . 4_666 ?
O4 W3 O9 Cs2 -139.50(8) . . . 3_667 ?
O10 W3 O9 Cs2 -48.20(9) . . . 3_667 ?
O6 W3 O9 Cs2 40.94(9) 3_767 . . 3_667 ?
O3 W3 O9 Cs2 129.90(8) . . . 3_667 ?
O1 W3 O9 Cs2 35.5(15) . . . 3_667 ?
Nb1 W3 O9 Cs2 -45.90(13) 3_767 . . 3_667 ?
Cs1 W3 O9 Cs2 175.82(7) 4_666 . . 3_667 ?
O9 W3 O10 Nb1 176.94(14) . . . 3_767 ?
O4 W3 O10 Nb1 -78.14(13) . . . 3_767 ?
O6 W3 O10 Nb1 77.80(13) 3_767 . . 3_767 ?
O3 W3 O10 Nb1 1.4(3) . . . 3_767 ?
O1 W3 O10 Nb1 0.50(10) . . . 3_767 ?
Cs2 W3 O10 Nb1 127.05(14) 3_667 . . 3_767 ?
Cs1 W3 O10 Nb1 -106.70(11) 4_666 . . 3_767 ?
O9 W3 O10 W1 176.94(14) . . . 3_767 ?
O4 W3 O10 W1 -78.14(13) . . . 3_767 ?
O6 W3 O10 W1 77.80(13) 3_767 . . 3_767 ?
O3 W3 O10 W1 1.4(3) . . . 3_767 ?
O1 W3 O10 W1 0.50(10) . . . 3_767 ?
Nb1 W3 O10 W1 0.0 3_767 . . 3_767 ?
Cs2 W3 O10 W1 127.05(14) 3_667 . . 3_767 ?
Cs1 W3 O10 W1 -106.70(11) 4_666 . . 3_767 ?
O9 W3 O10 Cs1 -12.0(2) . . . 3_667 ?
O4 W3 O10 Cs1 92.94(19) . . . 3_667 ?
O6 W3 O10 Cs1 -111.1(2) 3_767 . . 3_667 ?
O3 W3 O10 Cs1 172.46(18) . . . 3_667 ?
O1 W3 O10 Cs1 171.6(2) . . . 3_667 ?
Nb1 W3 O10 Cs1 171.1(3) 3_767 . . 3_667 ?
Cs2 W3 O10 Cs1 -61.87(17) 3_667 . . 3_667 ?
Cs1 W3 O10 Cs1 64.4(2) 4_666 . . 3_667 ?
O9 W3 O10 Cs2 49.88(11) . . . 3_667 ?
O4 W3 O10 Cs2 154.81(8) . . . 3_667 ?
O6 W3 O10 Cs2 -49.25(8) 3_767 . . 3_667 ?
O3 W3 O10 Cs2 -125.7(2) . . . 3_667 ?
O1 W3 O10 Cs2 -126.55(5) . . . 3_667 ?
Nb1 W3 O10 Cs2 -127.05(14) 3_767 . . 3_667 ?
Cs1 W3 O10 Cs2 126.25(6) 4_666 . . 3_667 ?
O14 Cs1 O11 Na1 -25.38(9) . . . 2_556 ?
O13 Cs1 O11 Na1 170.96(10) . . . 2_556 ?
O8 Cs1 O11 Na1 6.22(15) . . . 2_556 ?
O12 Cs1 O11 Na1 42.57(9) . . . 2_556 ?
O5 Cs1 O11 Na1 103.49(10) 1_455 . . 2_556 ?
O10 Cs1 O11 Na1 109.94(10) 3_667 . . 2_556 ?
O3 Cs1 O11 Na1 -93.14(9) 4_565 . . 2_556 ?
O4 Cs1 O11 Na1 -134.93(10) 4_565 . . 2_556 ?
Nb3 Cs1 O11 Na1 -122.42(8) 4_565 . . 2_556 ?
W3 Cs1 O11 Na1 -122.42(8) 4_565 . . 2_556 ?
O14 Cs1 O11 Cs2 163.05(8) . . . . ?
O13 Cs1 O11 Cs2 -0.61(14) . . . . ?
O8 Cs1 O11 Cs2 -165.35(7) . . . . ?
O12 Cs1 O11 Cs2 -129.00(8) . . . . ?
O5 Cs1 O11 Cs2 -68.08(7) 1_455 . . . ?
O10 Cs1 O11 Cs2 -61.63(6) 3_667 . . . ?
O3 Cs1 O11 Cs2 95.29(5) 4_565 . . . ?
O4 Cs1 O11 Cs2 53.50(5) 4_565 . . . ?
Na1 Cs1 O11 Cs2 -171.57(11) 2_556 . . . ?
Nb3 Cs1 O11 Cs2 66.00(4) 4_565 . . . ?
W3 Cs1 O11 Cs2 66.00(4) 4_565 . . . ?
O5 Cs2 O11 Na1 167.3(4) 4_465 . . 2_556 ?
O6 Cs2 O11 Na1 75.6(4) 1_455 . . 2_556 ?
O12 Cs2 O11 Na1 -104.0(4) 2_546 . . 2_556 ?
O16 Cs2 O11 Na1 48.4(6) . . . 2_556 ?
O4 Cs2 O11 Na1 -84.1(4) 4_565 . . 2_556 ?
O8 Cs2 O11 Na1 -143.7(4) 4_565 . . 2_556 ?
O10 Cs2 O11 Na1 38.6(4) 3_667 . . 2_556 ?
O15 Cs2 O11 Na1 -10.9(4) . . . 2_556 ?
O9 Cs2 O11 Na1 102.5(4) 3_667 . . 2_556 ?
Na1 Cs2 O11 Na1 -47.4(4) . . . 2_556 ?
W3 Cs2 O11 Na1 73.8(4) 3_667 . . 2_556 ?
O5 Cs2 O11 Cs1 -166.62(6) 4_465 . . . ?
O6 Cs2 O11 Cs1 101.66(6) 1_455 . . . ?
O12 Cs2 O11 Cs1 -77.94(9) 2_546 . . . ?
O16 Cs2 O11 Cs1 74.4(3) . . . . ?
O4 Cs2 O11 Cs1 -58.03(6) 4_565 . . . ?
O8 Cs2 O11 Cs1 -117.66(9) 4_565 . . . ?
O10 Cs2 O11 Cs1 64.65(6) 3_667 . . . ?
O15 Cs2 O11 Cs1 15.17(9) . . . . ?
O9 Cs2 O11 Cs1 128.60(10) 3_667 . . . ?
Na1 Cs2 O11 Cs1 -21.35(12) . . . . ?
W3 Cs2 O11 Cs1 99.88(5) 3_667 . . . ?
O14 Cs1 O12 Na1 39.87(8) . . . 2_556 ?
O13 Cs1 O12 Na1 -176.44(10) . . . 2_556 ?
O8 Cs1 O12 Na1 115.16(9) . . . 2_556 ?
O11 Cs1 O12 Na1 -40.40(9) . . . 2_556 ?
O5 Cs1 O12 Na1 -166.02(9) 1_455 . . 2_556 ?
O10 Cs1 O12 Na1 -113.91(10) 3_667 . . 2_556 ?
O3 Cs1 O12 Na1 31.13(12) 4_565 . . 2_556 ?
O4 Cs1 O12 Na1 -37.10(12) 4_565 . . 2_556 ?
Nb3 Cs1 O12 Na1 -2.81(17) 4_565 . . 2_556 ?
W3 Cs1 O12 Na1 -2.81(17) 4_565 . . 2_556 ?
O14 Cs1 O12 Cs2 93.8(4) . . . 2_556 ?
O13 Cs1 O12 Cs2 -122.5(3) . . . 2_556 ?
O8 Cs1 O12 Cs2 169.1(4) . . . 2_556 ?
O11 Cs1 O12 Cs2 13.5(3) . . . 2_556 ?
O5 Cs1 O12 Cs2 -112.1(4) 1_455 . . 2_556 ?
O10 Cs1 O12 Cs2 -60.0(3) 3_667 . . 2_556 ?
O3 Cs1 O12 Cs2 85.0(4) 4_565 . . 2_556 ?
O4 Cs1 O12 Cs2 16.8(4) 4_565 . . 2_556 ?
Na1 Cs1 O12 Cs2 53.9(3) 2_556 . . 2_556 ?
Nb3 Cs1 O12 Cs2 51.1(4) 4_565 . . 2_556 ?
W3 Cs1 O12 Cs2 51.1(4) 4_565 . . 2_556 ?
O13 Cs1 O14 Na1 -173.06(12) . . . 2_556 ?
O8 Cs1 O14 Na1 -132.28(10) . . . 2_556 ?
O11 Cs1 O14 Na1 25.50(9) . . . 2_556 ?
O12 Cs1 O14 Na1 -42.21(9) . . . 2_556 ?
O5 Cs1 O14 Na1 -78.09(12) 1_455 . . 2_556 ?
O10 Cs1 O14 Na1 -17.73(11) 3_667 . . 2_556 ?
O3 Cs1 O14 Na1 131.11(10) 4_565 . . 2_556 ?
O4 Cs1 O14 Na1 91.75(9) 4_565 . . 2_556 ?
Nb3 Cs1 O14 Na1 121.01(8) 4_565 . . 2_556 ?
W3 Cs1 O14 Na1 121.01(8) 4_565 . . 2_556 ?
O16 Na1 O15 Na1 107.78(13) . . . 3_557 ?
O14 Na1 O15 Na1 32.9(6) 2_546 . . 3_557 ?
O11 Na1 O15 Na1 -84.12(11) 2_546 . . 3_557 ?
O12 Na1 O15 Na1 -167.92(12) 2_546 . . 3_557 ?
O15 Na1 O15 Na1 0.0 3_557 . . 3_557 ?
Cs2 Na1 O15 Na1 164.30(11) . . . 3_557 ?
Cs1 Na1 O15 Na1 -109.39(14) 2_546 . . 3_557 ?
O16 Na1 O15 Cs2 -56.52(10) . . . . ?
O14 Na1 O15 Cs2 -131.4(6) 2_546 . . . ?
O11 Na1 O15 Cs2 111.59(10) 2_546 . . . ?
O12 Na1 O15 Cs2 27.78(10) 2_546 . . . ?
O15 Na1 O15 Cs2 -164.30(11) 3_557 . . . ?
Na1 Na1 O15 Cs2 -164.30(11) 3_557 . . . ?
Cs1 Na1 O15 Cs2 86.31(13) 2_546 . . . ?
O5 Cs2 O15 Na1 33.91(12) 4_465 . . . ?
O6 Cs2 O15 Na1 120.72(9) 1_455 . . . ?
O12 Cs2 O15 Na1 -21.14(8) 2_546 . . . ?
O16 Cs2 O15 Na1 46.75(10) . . . . ?
O4 Cs2 O15 Na1 -84.15(9) 4_565 . . . ?
O8 Cs2 O15 Na1 -88.21(12) 4_565 . . . ?
O10 Cs2 O15 Na1 170.13(10) 3_667 . . . ?
O9 Cs2 O15 Na1 156.43(8) 3_667 . . . ?
O11 Cs2 O15 Na1 -148.08(8) . . . . ?
W3 Cs2 O15 Na1 148.85(7) 3_667 . . . ?
O5 Cs2 O15 Na1 -24.6(4) 4_465 . . 3_557 ?
O6 Cs2 O15 Na1 62.2(4) 1_455 . . 3_557 ?
O12 Cs2 O15 Na1 -79.7(4) 2_546 . . 3_557 ?
O16 Cs2 O15 Na1 -11.8(3) . . . 3_557 ?
O4 Cs2 O15 Na1 -142.7(4) 4_565 . . 3_557 ?
O8 Cs2 O15 Na1 -146.7(3) 4_565 . . 3_557 ?
O10 Cs2 O15 Na1 111.6(4) 3_667 . . 3_557 ?
O9 Cs2 O15 Na1 97.9(4) 3_667 . . 3_557 ?
O11 Cs2 O15 Na1 153.4(3) . . . 3_557 ?
Na1 Cs2 O15 Na1 -58.5(4) . . . 3_557 ?
W3 Cs2 O15 Na1 90.3(4) 3_667 . . 3_557 ?
O14 Na1 O16 Cs2 -131.77(10) 2_546 . . . ?
O11 Na1 O16 Cs2 12.0(5) 2_546 . . . ?
O15 Na1 O16 Cs2 60.71(10) . . . . ?
O12 Na1 O16 Cs2 -48.54(9) 2_546 . . . ?
O15 Na1 O16 Cs2 148.25(9) 3_557 . . . ?
Na1 Na1 O16 Cs2 105.05(8) 3_557 . . . ?
Cs1 Na1 O16 Cs2 -87.91(12) 2_546 . . . ?
O5 Cs2 O16 Na1 120.85(11) 4_465 . . . ?
O6 Cs2 O16 Na1 -143.47(10) 1_455 . . . ?
O12 Cs2 O16 Na1 41.27(9) 2_546 . . . ?
O4 Cs2 O16 Na1 12.11(12) 4_565 . . . ?
O8 Cs2 O16 Na1 80.65(14) 4_565 . . . ?
O10 Cs2 O16 Na1 -106.41(9) 3_667 . . . ?
O15 Cs2 O16 Na1 -48.26(9) . . . . ?
O9 Cs2 O16 Na1 -160.72(8) 3_667 . . . ?
O11 Cs2 O16 Na1 -115.1(3) . . . . ?
W3 Cs2 O16 Na1 -138.28(7) 3_667 . . . ?



loop_

_geom_hbond_atom_site_label_D

_geom_hbond_atom_site_label_H

_geom_hbond_atom_site_label_A

_geom_hbond_distance_DH

_geom_hbond_distance_HA

_geom_hbond_distance_DA

_geom_hbond_angle_DHA

_geom_hbond_site_symmetry_A















O11 H11A O9 1.00(2) 2.21(10) 2.821(4) 118(8) 3_667
O11 H11A O10 1.00(2) 2.51(7) 3.362(4) 142(9) 3_667
O11 H11B O8 0.991(19) 1.96(3) 2.904(4) 158(5) 4_565
O12 H12A O7 0.99(2) 2.37(9) 3.150(4) 135(9) 3_667
O12 H12A O4 0.99(2) 2.43(6) 3.318(4) 149(9) 3_667
O12 H12A O10 0.99(2) 2.43(8) 3.196(4) 134(8) 3_667
O12 H12B O7 0.99(2) 1.89(5) 2.803(4) 152(8) .
O13 H13A O9 0.99(2) 2.11(5) 2.976(4) 146(6) 2_647
O13 H13B O9 0.99(2) 1.73(3) 2.689(4) 162(7) 4_565
O14 H14A O5 1.00(2) 1.95(3) 2.944(4) 169(8) 4_565
O14 H14B O6 0.99(2) 1.75(2) 2.728(4) 171(7) .
O15 H15A O2 1.00(2) 1.92(5) 2.856(4) 154(9) 1_455
O15 H15B O13 1.00(2) 1.77(4) 2.750(5) 163(12) .
O16 H16A O3 1.00(2) 1.83(5) 2.732(4) 149(8) 4_465
O16 H16B O8 0.989(19) 1.97(2) 2.942(4) 169(6) 1_455



_diffrn_measured_fraction_theta_max 1.000

_diffrn_reflns_theta_full        40.00

_diffrn_measured_fraction_theta_full 1.000

_refine_diff_density_max         2.644

_refine_diff_density_min         -1.995

_refine_diff_density_rms         0.303

